Abstract
Plasmonics and metamaterials have attracted considerable attention over the past decade, owing to the revolutionary impacts that they bring to both the fundamental physics and practical applications in multiple disciplines. Although the two fields initially advanced along their individual trajectories in parallel, they started to interfere with each other when metamaterials reached the optical regime. The dynamic interplay between plasmonics and metamaterials has generated a number of innovative concepts and approaches, which are impossible with either area alone. This review presents the fundamentals, recent advances, and future perspectives in the emerging field of plasmonic metamaterials, aiming to open up new exciting opportunities for nanoscience and nanotechnology.
1 Introduction
Since the early 2000s, metamaterials have emerged as a new frontier of science involving physics, material science, engineering, optics, and nanoscience. The primary reason for the extensive interest in metamaterials lies in the fact that metamaterials have implemented a wide range of exceptional properties by engineering the internal physical structures of their building blocks. This is distinctly different from natural materials, whose properties are primarily determined by the chemical constituents and bonds.
Metamaterials comprise periodically or randomly distributed artificial structures with the size and spacing much smaller than the wavelength of interest [1–4]. From the deep subwavelength feature, the microscopic detail of each individual structure cannot be resolved by the electromagnetic waves. We can homogenize the assembly of these inhomogeneous elements, and assign effective material properties at the macroscopic level [5]. Importantly, the effective material properties are predominantly determined by the size, shape, or structure of the building blocks of metamaterials, instead of the intrinsic properties of the constituent materials that are used to construct metamaterials. Using different metamaterial designs (Figure 1), researchers have been able to engineer the material properties with unprecedented degrees of freedom and have demonstrated extremely lowfrequency plasmons [6], artificial magnetism [7], negative refractive index [8], extremely large refractive index [9], and strong chirality [10]. The broad spectrum of material properties offered by metamaterials also propels the rapid development of transformation optics, which enables us to manipulate the flow of electromagnetic waves in almost arbitrary manners [11–15].
Figure 1
After the proofofprinciple experiments in the microwave regime, the operation frequency of metamaterials was quickly pushed to higher frequency from the terahertz (THz) to mid/nearinfrared and to visible [16]. Because most metamaterials are composed of metals, the plasmonic effect of metals plays an important role in optical metamaterials. For example, the magnetic resonance frequency of splitring resonators (SRRs) inversely scales with the structural dimension when the operation frequency is below ∼100 THz, where the metal can still be treated as a perfect metal with infinite carrier density and zero carrier velocity [4, 17]. However, this scaling law breaks down when approaching the optical regime, and the model for real metals must be adopted. At optical frequencies, the kinetic energy of electrons can no longer be neglected comparing with the magnetic field energy driving the current in the loop, which contributes an additional term to the inductance of SRRs [18, 19]. This electron inertia together with other plasmonic effects changes the simple scaling law in a complicated way, leading to an ultimate saturation of resonance frequencies of SRRs at about several hundred THz. Therefore, a more comprehensive exploration of plasmonic effects in metals will construct a solid foundation to develop optical metamaterials.
Plasmonics research focuses on the unique properties and applications of surface plasmon polaritons (SPPs), quasiparticles arising from the strong interaction between light and free electrons in metals [20, 21]. At the interface between a semiinfinite metal and a semiinfinite dielectric, SPPs behave as a surface wave that propagates along the interface while exponentially decaying into both the dielectric and metal (Figure 2A and B). The dispersion relation of SPPs at a dielectricmetal interface can be obtained by solving Maxwell’s equations and applying proper boundary conditions. Denoting the dielectric constant of the metal and the dielectric material as ε_{m} and ε_{d}, respectively, the dispersion relation of surface plasmons is written as
Figure 2
where ω is the angular frequency, c is the speed of light in vacuum, and k_{z} is the wave vector of SPPs along the propagation direction (zaxis). Figure 2C plots the dispersion relation for SPPs at the silverair interface. The dielectric constant ε_{m} of silver is a frequencydependent function given by the Drude model,
The fundamentals, developments, and applications of metamaterials and plasmonics have been discussed in many review articles. However, they focus on either metamaterials or plasmonics, rather than the remarkable properties and effects originating from the interplay between these two areas. As demonstrated by a number of groups, combining metamaterials and plasmonics could open up a broad range of opportunities to advance both fields and stimulate new crossdisciplinary approaches. Therefore, it is time to review the recent progress in plasmonic metamaterials. It is beneficial to reflect how the concepts of metamaterials inspire plasmonics and vice versa, potentially creating more breakthroughs in both areas, and in nanotechnology in a broader context.
The rest of the review is organized as follows. We will first discuss different schemes to realize negative refractive index and negative refraction at optical frequencies, followed by the review of recently developed metasurfaces that allow us to generalize the refraction and reflection laws by controlling the phase front. Subsequently, we will present THz plasmonics and metamaterials based on graphene, which exhibit extraordinary tunability via electrical gating. One important application of plasmonic metamaterials is biomedical sensing, which will be presented in Section 5. We will then discuss some selfassembly techniques to implement sophisticated plasmonic metamaterials with fine features and, finally, provide a conclusion and a brief perspective on the fascinating area of plasmonic metamaterials.
2 Plasmonic metamaterials to implement negative refraction and negative refractive index
Negative refractive index and negative refraction are the primary incentive that kindled the research of metamaterials. In 1968, Victor G. Veselago, a Russian physicist, published a theoretical paper studying a material with a negative refractive index [32]. He showed that if the relative electric permittivity (ε_{r}) and relative magnetic permeability (μ_{r}) are simultaneously negative, the refractive index of the material has to be negative as well, that is,
Such a negativeindex material (NIM) does not exist in nature, but it exhibits many remarkable properties. For instance, it can be rigorously proven from Maxwell’s equations that for a plane wave propagating in a NIM, the wave vector
The unusual electromagnetic properties of NIMs prompt us to revisit some fundamental phenomena. For example, it is found that Snell’s law, Doppler effect, Cherenkov effect, and radiation pressure are all reversed in NIMs [32]. Let us focus on Snell’s law, one of the basic laws in electromagnetics that determines how light refracts at the interface between two media. As illustrated in Figure 3A, if light is incident from a positiveindex material to a negativeindex one, the refracted light lies on the same side as the incident light with respect to the surface normal. This is because the tangential components of the wave vectors for incident and refracted light have to be conserved, and the energy must flow away from the interface (causality principle). From Snell’s law
Figure 3
the angle of refraction is indeed negative when the refractive indices of the two materials are opposite in signs. In other words, negative refraction takes place.
With arrays of copper wires and split ring resonators to implement simultaneously negative permittivity and permeability (Figure 3B), negative index materials and negative refraction were first demonstrated experimentally at microwave frequencies [8, 33]. This breakthrough sparked a global interest in metamaterial research. Tremendous effort has been devoted to scale down the size of the building blocks and optimize the metamaterial design to enable operation at higher frequencies. In order to work at optical frequencies, the feature size of metamaterials needs to be sub100 nm or even smaller, imposing a considerable fabrication difficulty. So far, the most successful optical NIMs are the fishnet structure [35], which significantly eases the fabrication burden. The fishnet metamaterials consist of two layers of metal meshes separated by a dielectric spacer layer. The paired stripes oriented parallel to the electric field provide negative permittivity, while the other pairs of stripes parallel to the magnetic field offer negative permeability. Such a configuration is much simpler than NIMs by combining metallic wires and split ring resonators. By stacking 11 functional layers of fishnet structures (Figure 3C), Xiang Zhang’s group demonstrated negative refraction through broadband, bulk, and lowloss NIMs at nearinfrared wavelengths [34]. Subsequently, lossfree and active optical NIMs in the visible wavelength range are achieved by incorporating gain materials into the fishnet structure [36].
Engineering the dispersion of SPPs provides an alternative approach to realize negative refraction and NIMs. For instance, there are two boundSPP modes in a twodimensional (2D) metaldielectricmetal (MDM) slab waveguide, which originate from the coupling and hybridization of the SPP mode at each individual metaldielectric interface when the thickness of the dielectric layer is small [37]. Interestingly, for the highfrequency, antisymmetric SPP mode (between the surface plasmon resonance frequency and the bulk plasmon frequency), the dispersion curve exhibits a negative slope, leading to negative group velocity (v_{g}=dω/dk). In contrast, the phase velocity (v_{p}=ω/k) is positive. As a result, the energy and phase fronts propagate in opposite directions; this mode thus behaves as if it has a negative refractive index. On the other hand, the lowfrequency, symmetric SPP mode (below the surface plasmon resonance frequency) appears to have a positive refractive index, as its group and phase velocities are simultaneously positive. Utilizing these properties, Lezec et al. directly demonstrated negative refraction at visible wavelengths by cascading two MDM waveguides [38]. The AuSi_{3}N_{4}Ag waveguide is designed to sustain a single negativeindex mode, while the AgSi_{3}N_{4}Ag waveguide is tailored to support propagation of only positive index modes within the same wavelength range (Figure 4A). The left column of Figure 4B shows the scanning electron microscope (SEM) image of the fabricated structure to demonstrate inplane negative refraction, which was made by applying a sequence of thermal evaporation and focused ion milling steps to both sides of a suspended Si_{3}N_{4} membrane. The input slit at the backside is revealed by electron transparency. In the prism region, the SPPs exhibit negative group velocity for the thickness of the Si_{3}N_{4} equal to 50 nm, while the rest region only sustains SPPs with positive group velocity. The semicircular slit works as an output coupler. At λ_{0}=685 nm, the position of the output spot indicates positive refraction at the prism’s interface with a refraction angle θ=+0.1°. The outputspot position shifts upward when λ_{0} is reduced to 514 nm, indicating negative refraction of SPPs with a refraction angle θ=43.7°. Given the incident angle equal to 7°, Snell’s law yields an effective index ratio for SPPs, which is +0.01 and 5.57 at λ_{0}=685 nm and 514 nm, respectively.
Figure 4
By stacking an array of MDM waveguides, Verhagen et al. theoretically demonstrated a metamaterial that has a 3D negative refractive index at visible frequencies [39]. In the design, the unit cell is a pair of strongly coupled MDM waveguides, in which eigenmodes resemble even and odd superpositions of the antisymmetric mode in the individual MDM waveguide. The odd superposition exhibits a negative mode wave vector as well as a negative coupling coefficient, resulting in negative refraction of both phase and energy for the transverse magnetic (TM) polarized light. The constant frequency contour can be almost spherical by tailoring the dielectric layer thickness between the unit cells. Therefore, wave propagation in such a 3D metamaterial can be described by an isotropic negative refractive index. Figure 4C and D show the H_{y} component when a TMpolarized plane wave (λ_{0}=400 nm) is incident from air into the metamaterial under two different conditions, that is, from the side and top of the waveguides, respectively. The arrows indicate the calculated timeaveraged Poynting vector
The negative refraction in Refs. [38] and [39] only works under TM polarization. To realize polarizationindependent or even isotropic NIMs, different approaches have been proposed. For example, similar to the planar MDM plasmonic waveguide, a coaxial MDM waveguide geometry can also support an antisymmetric SPP mode that has a negative refractive index (Figure 4E) [40]. Thanks to the cylindrical symmetry, the negativeindex mode is accessible from free space, independent on polarization and incident angle. It is shown that an array of coupled plasmonic coaxial waveguides functions as a NIM working in the 450–500 nm spectral range with a figure of merit FOM=∣Re(n)/Im(n)∣∼8. Figure 4F plots the H_{y} component for a TMpolarized light (λ_{0}=483 nm) incident at 30°. The phase front is clearly refracted in the negative direction with an angle of 12.5° with respect to the interface normal, and the wave indeed propagates backward from the finitedifference timedomain (FDTD) simulation. Negative refraction based on arrays of metallic nanowires was experimentally demonstrated in 2008 [44], while the mechanism is the negative group index arising from the hyperbolic dispersion of such a metamaterial [45, 46].
In addition, various attempts have been made to achieve isotropic NIMs by utilizing the Mie resonance of coreshell nanostructures. From the Mie theory, a particle can support both electric and magnetic multipolar modes, and the electromagnetic scattering and extinction efficiencies of a particle originate from the contribution from all the modes. The magnetic dipole resonance is generally much weaker than the fundamental electric dipole mode, but it can be significantly enhanced in a structure made of highpermittivity materials [47–49], which include semiconductors such as silicon and germanium. Some properly designed coreshell structures exhibit negative refractive indices by overlapping the electric and magnetic resonance within the same spectral range. The metallic core provides the electric plasmon response, while the semiconductor shell is responsible for the strong magnetic resonance with negative permeability. Numerical simulations have shown that both coreshell nanowires and coreshell nanoparticles can implement NIMs operating in the nearinfrared regime [50–52]. Because both electric and magnetic responses are obtained from a single constituent, no special requirement is needed for the lattice arrangement of inclusions. In particular, NIMs constructed by coreshell nanoparticles exhibit isotropic and polarizationindependent properties, owing to the spherical symmetry of the constituents. Experimental demonstration of such NIMs has not been achieved yet, although strong magnetic response has been observed in a complex plasmonic coreshell geometry [53].
At the end of this section, let us briefly discuss the reversal of Cherenkov effect, Doppler effect, and radiation pressure in NIMs [32]. Cherenkov effect is the electromagnetic radiation of a charged particle when it travels through a medium faster than the phase velocity of light in that medium [54]. In conventional materials with positive refractive index, the radiation falls into an expanding cone in the forward direction of movement, whereas in NIMs, the direction of radiation is reversed to the backward side [32, 55]. Similarly, inverse Doppler effect occurs when observing a source moving in an NIM. The experimental observation of the two effects is more challenging than that of negative refraction. For the reversed Cherenkov radiation, its power reaches maximum in the ultraviolet region and drops rapidly with increasing wavelengths [56]. The currently available optical metamaterials are still quite lossy, not suitable for detecting the weak radiation signal. Even at microwave regime where both the fabrication and detection techniques are well developed, only recently have researchers reported the first successful observation of the reversed Cherenkov radiation [57], though some groups had previously presented analogous [58] and indirect evidence [59]. For the inverse Doppler effect, the main difficulty originates from the measurement of frequency shift inside the media. So far, there has been a few experimental demonstrations of inverse Doppler effect based on nonlinear transmission lines at THz [60] and photonic crystals with an effective negative refractive index at optical frequencies [61]. However, the demonstration of inverse Doppler effect by means of NIMs is still lacking.
Another intriguing while subtle subject related to NIMs is the negative radiation pressure or negative optical force. According to the prediction in Veselago’s pioneering paper, a light beam propagating in a NIM and impinging on a reflecting object exerts a momentum directed backward to the source [32], unlike in a conventional medium where the resulting momentum points to the direction leaving the source [62]. Therefore, light pressure on the object embedded in a NIM counterintuitively causes an attraction or a pulling force. However, because the centuryold debate on the definition of momentum of light in a dielectric medium [63–65], namely, the AbrahamMinkowski controversy, has not yet been settled, we need to pay special attention when dealing with the radiation pressure or optical force in NIMs [66, 67]. Some authors suggest that for NIMs, positive admittance and group refractive index, instead of negative phase refractive index, should be used as material parameters when radiation pressure is concerned. Under such a consideration, the radiation pressure in NIMs is not different from that in conventional materials [68]. The experimental confirmation on the direction of radiation pressure is even more difficult than that of the inverse Doppler effect, owing to the similar material property and detection issues. The force of light is normally very weak, thus, needs to be measured via the motion of small objects. Unfortunately, current optical metamaterials are solids, which prevent the movement of any objects [69]. Although the optical force verification in NIMs is intrinsically challenging, research on negative optical forces has recently achieved great progress by other judicious strategies, such as tailoring the incident beam profile [70, 71], the object morphology [70], and the dielectric environment [72]. All these experiments are performed based on materials with positive refractive index, which exceed the scope of this paper. For a more detailed discussion on negative optical forces, we refer the readers to a latest review article [73].
3 Plasmonic metasurfaces
Since 2011, there has been an extensive interest in metasurfaces, a new kind of 2D metamaterials [74–85]. By patterning plasmonic nanostructures and engineering the spatial phase distribution within the plane, we can achieve exotic optical phenomena and optical components, including negative refraction or reflection, as well as ultrathin focusing or diverging lenses. These findings are remarkable, as normally, a material with a finite thickness (with respect to the wavelength) is required to accumulate sufficient phase to shape the beam profile. This requirement applies to classical optical components (such as glass lenses, prisms, and wave plates) and also metamaterials (such as a NIM slab for imaging). In comparison, metasurfaces tailor the inplane phase front using an extremely thin slab consisting of judiciously designed plasmonic structures. To some extent, metasurface can be considered as the optical counterpart of frequency selective surface (FSS) [86], a 2D planar structure widely used in radiowave and microwave regions under the long wavelength limit. In FSS, each unit cell acts as a small antenna, which is excited by external incidence and then emits or scatters waves with a phase variation relative to its neighboring units. As a result, specifically tailored wavefronts can be realized. Depending on the characteristic of the scattered waves, an FSS can be used as a lens (transmitarray) [87, 88] a reflector (reflectarray) [89], or an absorber [90], etc. Thanks to the advances in nanotechnology, optical nanoantennas with a feature size below 100 nm can be routinely fabricated and precisely arranged. By rationally designing the structural features, one can build optical nanoantenna arrays analogous to FSS. These compact arrays introduce prescribed phase distribution within deep subwavelength thickness, leading to exceptional changes of light propagation characteristics. Here, we concentrate on the current development of nanoantennabased metasurfaces for controlling propagating waves and surface plasmons, while the application of metasurfaces for biosensing will be discussed in Section 5.
In conventional optical components consisting of dielectrics, the behavior of light is governed by the gradual phase change accumulated along the optical path, implying that the surface geometry and refractive index profile are the two most important factors. On the other hand, it is well known that phased arrays at radio frequencies, which utilize a group of antennas fed by spatially varied signals to control the radiation pattern, can introduce abrupt phase shifts along the optical path to steer electromagnetic waves. Similar active devices at optical wavelengths have long been investigated aiming at largescale onchip integration. A nanophotonic phased array was successfully fabricated recently [91]. For passive devices, as long as the change of phase occurs within a very small thickness, the effect of wave propagation in this layer can be neglected, making the phase discontinuity an inherent characteristic of the interface. Under this circumstance, the standard Snell’s law that characterizes refraction and reflection should be rewritten into a generalized form [74]:
where θ_{i}, θ_{t}, and θ_{r} are the angles of incidence, refraction, and reflection, respectively, n_{i} and n_{t} are the refractive indices of the two media on the incidence and transmission side, respectively, λ_{0} denotes the wavelength in free space, and ∇Φ is the gradient of phase along the interface. A nontrivial phase gradient will change the directions of the refracted and reflected light simultaneously. This feature is fundamentally different from bulk materials or even metamaterials, where normally only the direction of the refracted component is changed. In addition, as can be deduced from Eqs. (4) and (5), if the abrupt phase shift term ∇Φ is properly selected, not only negative refraction but also negative reflection can take place.
The physical realization of an interface with continuous phase shifts is not trivial. Fortunately, it can be constructed by an array of plasmonic nanostructures with varied geometries and subwavelength separations. Similar to the longwavelength counterparts of transmitarrays and reflectarrays in FSS, here, the spatially varied nanostructures play the role of resonators to engineer the inplane phase shifts, which eventually determine the directions of the refracted and reflected beams. Figure 5A shows the SEM micrograph of a metasurface consisting of gold nanoantennas with a V shape [74]. By breaking the geometrical symmetry, a Vshaped antenna gives different responses to the different polarization components of the incident light, providing a wide range of degrees of freedom to modify the phase distribution and the state of the scattered light at the interface. As shown in Figure 5A, the Vshaped nanoantennas are arranged periodically along the x direction (period 11 μm), and the angle between the axis of symmetry of each unit cell and the x/yaxis is fixed to be 45°. For an x or ypolarized incidence, these antennas can provide crosspolarized scattered light, with equal amplitudes and constant phase difference between neighbors along the xaxis. For the scattered light, the crosspolarized component exhibits anomalous reflection and refraction due to the phase discontinuity across the interface, while the other component simply follows the standard laws, resulting in ordinary propagation. Figure 5B plots the schematic of an experimental setup with ypolarized incidence. This 2D demonstration of anomalous refraction and reflection was later extended to the 3D version [92].
Figure 5
A novel application of metasurfaces is farfield beam shaping [84, 93–99]. Because phase shifts are controlled by the arrangement of plasmonic nanoantennas, the wave front of the scattered light can be shaped in an almost arbitrary manner. For example, one can easily generate light beams carrying desirable orbital angular momentum (OAM), socalled optical vortices or vortex beams [74]. A vortex beam is an optical field propagating with its wavefront twisted around the beam axis like a corkscrew. This unique property promises direct applications in detection [100] and optical tweezers [101, 102] for rotating or trapping small particles. The vortex beams have infinite states characterized by an integer called topological charge, which represents the number of twists of the wavefront as light propagates a distance of one wavelength. Because different topological charges correspond to different speeds of information manipulation, vortices are expected to be applied in signal processing such as encoding and multiplexing [103, 104]. The creation of vortex beams is commonly achieved by using spiral phase plates, computergenerated holograms, qplates, or other modulators, which are bulky and rely on the surface geometry and refractive index profile. In contrast, metasurface can easily generate such beams with a proper phase distribution by patterning nanoantenna arrays. The top left panel of Figure 5C shows an example of the fabricated plasmonic metasurface to create vortex beams at midinfrared with a topological charge of one. The array is divided into eight sectors occupied by one constituent element each, rendering, in turn, a π/4 phase delay in the clockwise direction. Using such a structure, vortex beams can be excited upon normal illumination of linearly polarized light. The resulting beam has a uniform intensity except the singularity at the center, which appears as a bright ring in the top right panel. The helical wave front of the vortex is revealed by its interference with copropagating Gaussian beams parallel and tilted with respect to it, as shown by the spiral and fringe patterns at the bottom of Figure 5C, respectively.
In addition to OAM, the spin angular momentum (SAM) is another fundamental property of light. In a circularly polarized light beam, each photon carries a SAM of
Metasurfaces exhibit three unique advantages over bulk metamaterials in controlling light propagation with extraordinary abilities. First, the reduced dimension could also reduce both loss and cost, which arises from Ohmic loss of metals and fabrication complexity, respectively. Second, the designs of nanoantennas are diverse, thus, allowing one to adopt different candidates for different applications, where the requirements on wavelength, polarization, and efficiency may vary. For instance, a dipole antenna array is demonstrated to work on the anomalous control of circularly polarized light [84, 94]. Last, the planar metasurface can be readily integrated with other onchip or quasiplanar optical devices. This is highly desirable for miniaturized photonic systems. Unlike conventional lenses with bulk volume and complex surface curvature, a metasurfacebased lens could be ultrathin, flat, and aberrationfree [84, 93, 111]. We note that recent progress at long wavelength regime is also impressive. In Ref. [112], a microwave metascreen is designed to tailor the wavefront without causing any reflection. This dual functionality is still challenging for the current metasurfaces based on nanoantennas [113].
Another exciting feature of plasmonic metasurfaces, which is revealed very recently, is the ability to control optical surface waves, such as SPPs, in the nearfield regime [76, 79–82]. Conceptually, one can manipulate the propagation of light and SPPs with the transformation optics approach as they both obey Maxwell’s equations [11, 12, 114–116]. However, the physical realization of transformation optical devices still relies on either bulk metamaterials or dielectrics in most cases, which leads to intrinsic limitations on the size and cost of the devices. The latest work by several groups shows that metasurfaces can efficiently mold SPPs [79–82]. The idea utilizes a fundamental nature of waves, even those bounded at interfaces, that the superposition of two waves may form complex power distribution owing to the constructive and destructive interference. When the patterned plasmonic nanostructures of a metasurface interact with light, part of the reradiative energy is converted to SPPs. In other words, the plasmonic nanostructures function as SPPs emitters. By controlling the relative phase among the emitters via modifying the geometry of the nanostructures or the polarization state of the incident light, one can achieve unidirectional excitation of SPPs.
The recent work of Capasso’s group uses an aperture array – the complementary structure of the nanoantennas, to excite directional SPPs [79]. As shown in Figure 6A, a single subwavelength aperture milled into a gold film resonantly interacts with light that is polarized along the long axis of the aperture, producing an equivalent dipole oriented along the short axis, as represented by the red arrow in the figure. The dipole excites SPPs, which display a symmetric radiation pattern. Then, in Figure 6B, the SPPs generated from a column of apertures with the same orientation interfere constructively along the planes parallel to the column, giving rise to planewavelike SPPs that propagate symmetrically away from the structure. By placing a second parallel column consisting of apertures oriented orthogonally to those in the first column, the total intensities of the leftgoing and rightgoing SPPs can be controlled by the helicity of the incident light and the separation of the two columns of apertures. The left panel of Figure 6C illustrates the SEM image of a metasurface with multiple column pairs to launch polarizationcontrolled SPPs. The right panels show that a linearly polarized light normally incident from top generates SPP beams of almost equal intensity to both sides of the structure, while in contrast, the right (left) circularly polarized light is converted to SPPs propagating to the right (left) side of the structure only. The different orientations of the apertures between a column pair are essential. The reason is similar to the previous work [74], in which the Vshaped antennas facilitate the coupling between plasmonic nanostructures and different field components. Nearfield interference can be also induced on a flat interface by a circularly polarized dipole, whose vertical and horizontal component owns an odd and even parity of spatial frequency spectrum, respectively, resulting in an asymmetric profile of SPPs. As proven in Ref. [80], a single slit obliquely illuminated by circularly polarized light can, indeed, excite directional SPPs as well.
Figure 6
An alternative route stems from the phase discontinuity mechanism. The metasurface consisting of an aperture array can provide a phase gradient as a dipole antenna array does. As we have discussed, this structure is able to control anomalous light propagation depending on the polarization state. When light illuminates on such an interface, the diffraction equation needs to be modified by taking into account the effect of the phase shifts [81]:
where θ_{t} and m are the angle and order of diffractions, respectively, s is the lattice constant of the array, and σ is a coefficient of helicity taking 1/1 for the left/right circular polarization. Figure 6D compares the ordinary and anomalous refraction and diffraction of two helicities at normal incidence. While the ordinary diffraction orders lie symmetrically about the surface normal, the anomalous ones are shifted sideward together with the refracted light in accordance with the helicity of the incidence. This asymmetric profile enables one side of the array to gain a larger wave vector, which leads to efficient excitation of SPPs. In contrast, the wave vector is smaller on the other side (shifted closer to the light line), and the SPP excitation condition is not satisfied.
One problem is the coupling efficiency of SPPs. The efficiency achieved in experiments was low, about 2.5% and 3.8% in Refs. [79] and [81], respectively. This can be improved by optimizing the array configuration and employing highly resonant structures. For instance, a compact magnetic resonator pair can generate directional SPPs with efficiency as high as 135% [117], enabling better conversion of light from free space to surface plasmons. With these recipes and better plasmonic materials, the coupling efficiency was enhanced up to 10∼14% in simulations and is expected to reach a higher level [81, 93].
The family of metasurfaces is actively growing, and there are several directions that might be worth exploring in the coming years. The symmetry property of nanoantennas is a possible gateway leading to highly efficient plasmonic sources and spincontrolled photonic devices. Hyperbolic metasurface inherits the superior ability of its 3D counterpart in terms of large photonic density of states [77, 118]. Therefore, they are promising for onchip lasing and quantum information applications. Other issues, like tunability, loss, and so forth, are also important aspects that always exist in plasmonic metamaterials.
4 Plasmonics and metamaterials based on graphene
Graphene, a monolayer of carbon atoms arranged in a honeycomb lattice [119, 120] has attracted a great deal of attention for plasmonics and metamaterials at terahertz and infrared frequencies [121–126]. The dispersion of conventional SPPs supported by noble metals approaches the light line in the long wavelength regime, and the subwavelength confinement is completely lost. However, graphene can support surface plasmons to confine light strongly while potentially maintaining small losses in this frequency range because of its unique electronic property [123, 127]. Moreover, the mechanical, electronic, optical, and even thermal properties of graphene are highly tunable via chemical doping and electrical gating [128–134]. These favorable features arouse enormous interests on the investigation of graphenebased tunable plasmonics and metamaterials.
Theoretically, surface plasmons can exist in a material with mobile charge carriers whose conductivity is predominantly imaginary [135]. This is equivalent to a material, such as a noble metal, of which the real part of electric permittivity is negative. Graphene is an atomically thin semiconductor, whose electron density, and thus the plasma frequency, is much lower than that of bulk noble metals. As a result, graphene satisfies the requirements of supporting SPPs as a bulk metal does, whereas its operating frequencies reside at terahertz and infrared regimes, much lower than that of metals at visible and ultraviolet. Because of the 2D nature of the platform, graphene surface plasmons exhibit exponential field decay into the surrounding dielectric layers on both sides of the graphene sheet (Figure 7A) [123]. Indeed, graphene plasmonics resemble plasmons in the 2D electron gases (2DEGs) that have been explored before [137–139].
Figure 7
As a zerogap semiconductor, graphene can be doped to high density of charge carriers by either chemical methods or varying the biased gate voltage. The latter approach, known as electrical gating, is particularly preferred as it provides an in situ and effective access to tune the electronic and optical properties of graphene layers [140–142]. Figure 7B illustrates one valley of the electronic band structure of graphene, where the intra and interband transitions are represented by the green and pink arrows, respectively. A sufficiently high level of doping leads to a larger value of Fermi energy E_{F}. The absorption of photons with energy less than 2E_{F} is forbidden due to the Pauli blocking. Therefore, doping can suppress the absorption losses introduced by the interband transition and compels SPPs toward higher frequencies [121, 124].
Because the charge carriers in graphene are massless, Dirac electrons and the excitations are essentially confined in the transverse dimension, graphene plasmons are expected to provide much smaller wavelengths and thereby much stronger lightmatter interaction. From the dispersion relation, one can calculate the SPPs wavelength on a graphene sheet, which is about 200 nm at infrared frequencies [127, 135], approaching two orders of magnitude smaller than the wavelength of illumination. Such an exceptional confinement is not possible in conventional SPPs supported by noble metals at the same frequency range. However, this feature brings a technical problem: the excitation and detection of graphene plasmons can hardly be efficient due to their large wave vector mismatch with photons in the free space. Although successful observations have been reported via electron spectroscopy [143, 144] and tunneling spectroscopy [145], the spectrally indirect probing is not sufficient to look into the underlying physics of graphene plasmons. Recently, two groups independently reported the direct spatial mapping of graphene plasmons based on the scatteringtype nearfield scanning optical microscopy (NSOM) [135, 136] at infrared frequencies. Thanks to the advanced experimental techniques, highresolution imaging of the realspace profiles of propagating and standing surface plasmons are achieved. Figure 7C shows the configuration of the experimental setup, which was employed in both studies. Plasmons with high inplane momenta are excited by illuminating a sharp atomic force microscope (AFM) tip with a focused infrared beam, as indicated by the green arrow. The nearfield amplitude profiles are obtained from the backscattered light beam (blue arrow). The tip is extremely sharp, with the curvature radius of around 25 nm, ensuring excitation of large momentum and high order of spatial resolution. The reported wavelength of graphene plasmons is about 200 nm, which is more than 40fold smaller than that of the incident infrared light. Various characteristics of SPPs can be observed from the resulting images. For instance, the plasmon interference patterns are given by the simulated nearfield amplitude profiles in Figure 7D. Because of the presence of the graphene/substrate boundary at L=0, interference occurs between the tiplaunched plasmons (white circles) and the reflected plasmons (green circles), giving rise to different standing wave patterns when the tip is located at a different distance from the edge, as denoted by the blue circles and arrows, respectively.
A unique property of graphene plasmonics is that the plasmon wavelength is determined by the carrier density, implying that one can tune the characteristics of graphene plasmons and achieve sophisticated functionalities by simply varying the gate bias [136]. Figure 7E shows the plasmonic switching by electrical gating, where tapered graphene ribbons are deposited on a SiO_{2} substrate with a Si backgate. As can be seen, with a sufficiently large and increasing backgate voltage V_{B}, which causes larger carrier density and Fermi energy, the two local plasmon modes shift toward regions with a larger ribbon width due to the corresponding increase in plasmon wavelength. This exciting result clearly manifests the effectiveness of graphene gate tuning and the capability of graphene plasmonics to control and switch optical signals at the nanoscale.
In addition to doping and gating, geometry patterning is an alternative approach to tune the optical properties of graphene, rendering a variety of graphenebased plasmonic and metamaterial structures at infrared wavelengths. The lightplasmon coupling in pristine graphene is relatively weak and not sufficient to serve practical devices. However, some recent experimental work demonstrated that rationally designed graphene patterns can dramatically enhance the coupling and improve the lightmatter interaction [140, 142, 146–149]. Therefore, patterning is an effective recipe to tune graphene plasmons, which not only diversifies the design of devices [125, 150–152] but also enables the investigation of the damping effect in graphene nanostructures [153]. As a representative example, graphene microribbon arrays are investigated in Ref. [140] and show interesting properties. The structure of a gated graphene ribbon array is shown in Figure 8A. The widths of ribbon and gap are identical and varied in experiments from 1 to 4 μm, which is much smaller than the wavelength of incidence and enables efficient excitation of plasmon resonances. Owing to the anisotropic nature of configuration, the microribbon array responds differently to incident light with polarization perpendicular and parallel to the ribbons. In Figure 8B, the spectra of perpendicular polarization exhibit a distinctly different Lorentz line shape because the plasmon excitations correspond to carrier oscillations across the width of microribbons. While the carrier concentration n increases with increasing gate voltages, the absorption peak not only gains strength but also shifts to a higher energy, in accord with the n^{1/4} scaling signature of massless Dirac electrons (Figure 8B). For comparison, the inset of Figure 8B depicts the absorption spectra for parallel polarization at three different gate voltages. In this case, the optical response originates from mobile charge carrier oscillation similar to that in a graphene monolayer, which can be described by Drude model and changes only in amplitude with increasing gate voltage. A noticeable fact is, in both cases, the absorption at plasmon resonances reaches the level of over 12% for gate voltage greater than 2 V. Compared with the 2.3% absorption by a single layer of pristine graphene [154], such a substantial absorption implies strong lightplasmon couplings in the patterned graphene ribbons.
Figure 8
For polarization perpendicular to the ribbons, changing the width of the ribbon is an alternative way to tune the plasmon resonance frequency. Figure 8C reports the change of normalized transmission with different ribbon widths w, in which the carrier concentration is fixed to be 1.5×10^{13} cm^{2}. Theoretical derivations based on quasistatic description suggest that the plasmon resonance scales as w^{–1/2}, a characteristic behavior of 2DEGs. The experimental results fit well with the prediction as indicated by the blueshifting trend of resonance with decreasing ribbon widths. Further engineering, such as broadening the ribbon width and adjusting the filling ratio, can be performed to achieve tunable plasmon resonance ranging from 1 to 10 THz.
The strong dependence of polarization may not be a desirable property in practical applications. Graphene/insulator stacks, in a circular shape and arranged in a highsymmetry order, can circumvent such a disadvantage [155]. More importantly, the number of the stacked layers significantly influences the plasmonic resonance frequency and amplitude [142, 156]. Figure 8D shows the SEM image of an array of microdisks arranged in a triangular lattice, where two parameters, the diameter of disks d and the lattice constant a, determine the configuration of the stack array in the transverse dimension. In Figure 8E, the extinction spectra of the samples are plotted for one, two, and fivelayer samples, respectively. With the increasing number of graphene layers, both the resonance frequency and peak intensity increase significantly because of the strong Coulomb interaction between adjacent layers, which is drastically different from the simple addition of carrier concentration in conventional 2DEG lattices. On the other hand, unlike resonances in graphene monolayer owning a weak n^{1/4} carrier density dependence, plasmons in the stack structure show a strongly enhanced dependence on carrier concentration. The resonance amplitude and frequency are proportional to n and n^{1/2}, respectively. The latter scale stands for conventional 2DEGs. As a result, one can effectively tune the resonance frequency and amplitude of the graphene plasmons in the stacked microdisks, promising great potential in THz photonic applications. By adjusting the inplane geometrical parameters while maintaining a large filling factor, which is defined as microdisk area over total area, a peak extinction as high as 85% can be achieved (red curve in Figure 8F). The device functions as a tunable, polarizationindependent plasmonic notch filter, and the peak value in the spectra corresponds to an extinction ratio of ∼8.2 dB.
Because of the extraordinary electronic properties and great tunability, graphene is regarded as a competitive candidate for many applications, such as absorbers [141], nanoantennas [151, 157, 158], and waveguides [125, 150, 159]. To further improve the performance of graphenebased devices, besides manipulation on graphene itself, like gating and patterning, the hybridization of graphene and other conventional plasmonic nanostructures or metamaterials is a promising direction. Such scenarios may generate a wide range of tunable optical devices at terahertz and infrared frequencies. For instance, Lee et al. recently demonstrated a tunable THz metamaterial by integrating metallic metaatoms with a gated graphene sheet [141, 160]. The schematic plot and optical micrograph of the fully integrated structure are shown in Figure 9A and B, respectively. To fabricate the sample, a graphene sheet grown by a chemical vapor deposition (CVD) process is transferred onto a hexagonal metaatom layer and connected to a grounded electrode. Thin metallic wire arrays are attached to both sides of the hybrid metamaterial as top and bottom electrode, which are designed to provide gate voltage while allowing light to transmit. The polarization of the incident terahertz wave should be perpendicular to the line electrodes in order to induce the extraordinary optical transmission (EOT) [161, 162]. Here, the metaatom layer plays a key role to enhance the electronic and optical properties of graphene by its strong resonance. The gatecontrolled lightmatter interaction can be interpreted as follows from two aspects: on one hand, the amplitude of onresonance transmission increases with increasing gate voltage, as the graphene layer becomes more conductive and suppress the intrinsic resonance of hexagonal metaatoms. On the other hand, the offresonance transmission acts in the reverse trend due to the gateinduced broadband absorption in graphene layer, which is dominated by the contribution of intraband transitions and, thus, cannot be reduced for larger gate voltage. Terahertz timedomain spectroscopy (THzTDS) [163] measurement reveals exceptional performance of the device. The amplitude of the transmitted wave is modulated up to 47% at the maximum gate voltage and system resonance frequency, as shown in Figure 9C. This result far exceeds the value of ∼30% achieved by metamaterialsemiconductor hybrid structures [141]. The functionality of phase modulation is relatively straightforward considering the resonant nature of the metaatoms. The maximum phase change is measured to be 32.2° at 0.65 THz (Figure 9D). Further improvement of both amplitude and phase modulation can be achieved when multilayers of graphene, instead of the single sheet, are integrated with metamaterials. The property of such hybridized graphene metamaterials strongly relies on the gate voltage. As seen from Figure 9E, the onresonance intensity transmission, reflection, and absorption traces exhibit three distinct scaling regimes from left to right, which correspond to the weak, linear, and sublinear dependence of the Fermi level on the voltage ∣∇V∣^{1/2}=∣V_{CNP}V_{g}∣^{1/2} (where V_{CNP} and V_{g} are the voltages of the charge neutral point and gate voltage, respectively) because of the conductivity variation of the graphene layer. Interestingly, this active graphene metamaterial also exhibits gatecontrolled optical hysteresis that can be applied to develop electrically controlled photonic memories. The design of the active metamaterials could be diverse as the richness of the metaatoms. In addition to tunable metamaterials, several groups have reported tunable plasmonics by graphene. The gatedependent dielectric properties of graphene enable the modulation of plasmon resonance frequency and quality factor. Successful demonstrations have been observed on nanoparticles [164], nanorods [165, 166], and bowtie resonators [167], etc., all of which are common building blocks to construct plasmonic devices.
Figure 9
The combination of graphene physics and plasmonics generates a versatile new platform for applications in the terahertz and optical regime. By maintaining the advantages of conventional plasmons, graphenebased devices are able to improve the performance of nanoantennas, broadband absorbers, and bio/chemicals while by keeping the ultrathin and highly tunable properties, they also have the potential to be used as building blocks of new emerging materials, such as hybrid metamaterials and metasurfaces. Along with the deeper insight of graphene plasmonics, we expect this branch of nanomaterials to bear more groundbreaking results.
5 Plasmonic metamaterials for biosensing
As discussed in the introduction, SPPs exhibit unique features of tight field confinement and strong field enhancement. They are very sensitive to the changes of refractive index of the dielectric media in the vicinity of metal structures. Taking advantage of these properties, one can design miscellaneous structures for sensing purposes [22, 168–172] through which observable changes of corresponding quantities, such as a shift in resonance [173–175], a variation in field intensity [155, 176], or an offset in angle [77, 177], are expected. Therefore, SPPs not only provide a labelfree, realtime access to probe biological components at nanoscales but also lead to an extremely high resolution. Both propagating and localized SPPs have been applied for biochemical or biomedical applications. They each have unique advantages while facing their own problems [173]. For approaches based on propagating SPPs, a detection sensitivity exceeding 10^{5} refractive index units (RIU) has been achieved. However, this target is still challenging for analytes with very small size or selective nanoarchitectures. As to localized SPPs, by altering the size, shape, and chemical components of the plasmonic structures, a device of this kind owns great tunability and adaptability, whereas it suffers a sensitivity of at least one order of magnitude lower.
Plasmonic metamaterials hold a new promise for biosensing with unprecedented sensitivity and specificity. On one hand, it inherits the feature of metamaterials that the operation frequency can be widely tuned to bind the characteristic vibrations of biomolecules, and the spectral line shape can be engineered to be very sharp to obtain higher sensitivity [176]. On the other hand, the plasmonic nanostructures serve as building blocks to keep the merit in adaptability, ensuring that the device satisfies the selective requirements in different applications. In this section, we briefly review recent advances in biosensing based on plasmonic metamaterials in four schemes, i.e., using Fano resonance, nanorod structures, metasurfaces, and chiral fields, respectively. From the limited space, we are not able to discuss other sensing approaches. Interested readers can refer to several latest pieces of work and reviews on these topics [178–182].
5.1 Fano resonance in plasmonic metamaterials
One recent research interest in plasmonic matamaterials is Fano resonance [176, 182–185]. Fano resonance is named after the Italian physicist Ugo Fano, who first suggested the theoretical explanation for the asymmetric scattering line shape of the inelastic scattering of electrons of helium [186]. Only until the recent decade was Fano resonance demonstrated in other systems. The origin of Fano resonance arises from the interference between a discrete narrow state and a wide continuum regardless of the nature of the system. Optical systems consisting of plasmonic nanostructures can be designed to achieve Fanolike spectral responses, which are suitable candidates for sensing, switching [187, 188], and lasing applications [189], etc.
Fano resonance exists in a variety of plasmonic structures and metamaterials. For example, it can occur through the light scattering from a metallic nanoparticle [184, 190]. According to the Mie theory, the scattering amplitudes of a nanoparticle involve multipolar resonant terms for both electric and magnetic responses, which correspond to different localized SPP modes. As the fundamental mode, the electric dipolar resonance is broadband and always the dominant term at low frequencies. However, higherorder modes, originating from the quadrupole, octupole, and so forth, become significant when the frequency increases. These highorder resonances are narrowband, thus, satisfying the condition of Fano resonance when they are coupled to the dipolar mode. Figure 10A plots the forward and backward scattering diagrams of a plasmonic nanoparticle, which show distinctly different features for the first two eigenmodes. The radius of the nanoparticle a is much smaller than the wavelength at dipolar resonance λ (a/λ=0.083), which ensures that the magnetic resonances are negligible, and only the electric resonances need to be considered. Constructive and destructive interference occurs near the quadrupolar resonance, rendering the line shape of the spectrum a typical, sharp asymmetric Fano profile. Further connection to biosensing is straightforward [182]. The scattered field intensity in the vicinity of the quadrupolar resonance changes so dramatically that even a slight detuning of frequency will induce astonishing transformation in the scattering patterns, as shown in Figure 10B. This sensitivity is highly desirable in sensing situations to probe the tiny refractive index change.
Figure 10
In coupled nanostructures, Fano resonance is observable from the scattering spectra as long as the size of the system is appropriate. For a single nanoparticle, interference occurs between the “bright” dipole and “dark” higherorder multipoles of the particle itself. Herein, by contrast, each metaldielectric interface supports a set of resonances, and both superradiant (bright) and subradiant (dark) states originate from the complex coupling of them, with individual plasmons oscillating in phase and out of phase, respectively. Normally, the dipoledipole coupling dominates the response of symmetric structures such as a nanoshell. However, to achieve Fano resonance for larger field enhancement and better spectral tunability, one needs to break the symmetry exciting higherorder multipolar modes [23, 191–197]. A representative example [191] is shown in Figure 10C and D, where the extinction spectra for normal incidence are calculated for nonconcentric ring/disk cavities with partial and complete filling of different dielectric insertions, respectively. For each curve, results of charge density calculation reveal that the narrow resonance at long wavelength is due to the antisymmetric alignment of the dipolar modes in the disk and ring, while the Fano profile around 1500 nm comes from the interaction between the quadrupolar ring mode and the broadband dipolar disk mode. Both spectra exhibit noticeable red shifts sensitive to the dielectric permittivity increase, and further comparison proves that the Fano resonance in the complete filling cavity provides the largest figure of merit for sensing. Such nanocavities are highly tunable in design, involving various planar configurations such as ring/disk dimmers [191], asymmetric split rings [193], and dolmenstyle slabs [194]. In particular, the latter gives a sharp resonance and is often used in plasmoninduced transparency, a plasmonic analog of the electromagnetically induced transparency (EIT) in atomic physics [195, 196].
Combining the advantages of sharp spectral response, large field enhancement, and tunable frequency of operation at infrared, Fano resonance in plasmonic metamaterials is a promising approach for biosensing applications. For instance, Wu et al. successfully demonstrated Fanoresonant asymmetric metamaterials for multispectral biosensing of nanometerscale monolayers of recognition proteins and their surface orientation [176]. As shown in Figure 11, similar to the dolmenstyle slabs, the FRAMM consists of three nanobar antennas, of which two are parallel and identical, and the third is perpendicularly attached to one of them serving as a symmetrybreaking coupler. The super and subradiant modes contributing to the Fano interference arise from the parallel (in phase) and antiparallel (out of phase) charge oscillations in the two identical branches (Figure 11A). In measurements, when protein nanolayers are immobilized on the surface of the FRAMM, the optical effect of each monolayer is equivalent to a dielectric film of the same thickness, which induces a spectral shift and intensity difference in the reflectivity spectrum with a unique fingerprint. The topmost protein monolayer can be detected and characterized by measuring the difference of reflectivity between substrates before and after the bonding process. Thereby, in principle, a structurespecific biosensing can always be accomplished by using the FRAMM substrate with recognition protein immobilized on its surface. Figure 11B illustrates the sensing concept schematically. A monolayer of protein A/G is immobilized on the surface of the FRAMM substrate as recognition moiety, and IgG antibodies are the target molecules to bond to the protein A/G. Comparisons of the experimental spectra before and after bonding of IgG are shown in Figure 11C with dashed and solid curves, respectively. For all the three FRAMMs with different resonant peaks, which are tuned either away from or precisely matching with the eigenfrequency of a biomolecule’s vibrational modes, the bonding of IgG changes reflectivity in evidently detectable amplitude. Highly specific information including the thickness and orientation of the bonding biomolecules can be derived with nanometerscale accuracy from the measured results at different resonances.
Figure 11
5.2 Nanorod metamaterials
In terms of biosensing using localized SPPs, various nanoparticle shapes like spheres, rings, ellipsoids, and rods are adopted. Among these candidates, nanorods, which possess relatively high sensitivity on refractive index changes and geometrical tunability, have been investigated most intensively [198]. Figure 12A shows the basic schematic of a nanorodbased immunoassay [199]. The nanorods are fixed on a glass substrate and coated with selfassembled monolayers (SAMs). The individual nanorod is about 15 nm in diameter and 50 nm long. To perform sensing, capture antibodies are precoupled to the SAMs, and specific antigens in the analyte solution will bind to them during the measurement. The extinction peak responds to this reaction with a spectral shift, which is relevant to the concentration of the target analyte and can be monitored via realtime analysis, as shown in Figure 12B. According to the tested results, this design yields a detection sensitivity of 170 nm per RIU and an FOM of 1.3.
Figure 12
Plasmonic metamaterials made of an array of nanorods can introduce new modes to serve as the performer of detection [200], which are expected to overcome the sensitivity limit of sensors based on localized SPPs and provide better adaptability. Recently, Kabashin et al. demonstrated a neat prototype by using an assembly of parallel Au nanorods (Figure 12C) [173], which are electrochemically grown in a porous, anodized alumina template. The structural parameters are highly tunable during fabrication, with rod lengths ranging from 20 to 700 nm, diameters from 10 to 50 nm, and separations from 40 to 70 nm, respectively. From the viewpoint of metamaterials, this subwavelength nanorod array behaves as a bulk material with unusual hyperbolic dispersion relation, whose permittivity tensor contains a negative component along the long axis of nanorods and positive components along the short axis. With this unique feature, although the field distribution in the porous layer is determined by plasmonmediated interaction between nanorods, the whole structure supports a guided photonic mode at near infrared. The excitation condition of this guided mode is similar to excite SPPs on a metal film, that is, TM polarization and attenuated total reflection (ATR). For isolated nanorods with a sufficiently large separation distance, the nearfield coupling is negligible and usually it is the localized SPPs that dominate the response. On the other hand, the guided mode arising from the collective plasmonic response in the nanorod metamaterial is able to reach an extremely high sensitivity of 32,000 nm per RIU and a FOM of 330, far exceeding those of sensors based on localized SPPs, and even propagating SPPs.
Another intrinsic advantage of the nanorod metamaterialbased sensor is its porous texture, which not only tremendously increases the surface area for reaction but also helps to achieve a large probing depth. Figure 12C displays the schematic of the flow cell, where the inset shows the field profile of the guided mode in crosssection. The nanorods are preliminarily immobilized with streptavidin molecules for functionalization. In the experiment, PBS buffer solution and biotin of different concentrations are pumped through the nanorod array (green wide arrows), and reflectivity is measured below the substrate with the ATR configuration. Figure 12D shows the realtime response of such a sensor to the reaction of biotinstreptavidin binding. Considering the small molecular weight of biotin, the fast and large resonant dip shift after the analyte injection is truly remarkable. This strongly indicates the power of the guided mode of nanorod metamaterials for biosensing. Noticeably, the modern technique of nanofabrication is mature in processing nanorod/wire structures, which allows them to be integrated into complex systems for different applications and requirements.
5.3 Plasmonic metasurfaces
The metasurface discussed in section 3 could also open a new route for biosensing designs. Although SPPs are best known for their tremendous local field enhancement, the absolute reading of intensity variations has some intrinsic limitations in satisfying the high precision requirement of quantitative analysis. In practice, normally, a spectral shift in resonance is more preferred as a metric parameter. Owing to the ability of causing anomalous reflection and refraction, the plasmonic metasurface can translate tiny refractive index changes at local positions into measurable offsets in the angle of the reflected or refracted beam [77]. In this way, one can produce ultrasensitive biosensors relying on the angle offset as schematically illustrated in Figure 13A.
Figure 13
Another measurable parameter that has been adopted in biochemical or biomedical detection is the phase of light. Specifically, it is the socalled “singular phase”, [177], which refers to the extremely fast phase changes where the intensity of light becomes very close to zero. The corresponding detection can be realized with the help of plasmonic metasurfaces by measuring the reflected light beams. As it is demonstrated that the point of zero reflection exists in a variety of periodic nanostructures with only slightly different wavelengths, the design of the unit cells is flexible and not sensitive to their topologies. Figure 13B illustrates the schematic of biosensing based on a plasmonic doublenanodot array on a glass substrate. The array constant a=320 nm, average size of the dots d=135 nm, and dot separation of the pairs s=140 nm. To perform measurements, biotin is attached to the functionalized nanodots, which are represented by the dark green triangles and golden truncated cones, respectively. The metasurface is exposed to streptavidin solutions, in which the target biomolecules are denoted by the red pie chartlike disks. Light illuminates the array in the ATR geometry, and localized SPPs of the nanodots are coupled by the diffracted wave propagating along the surface, as shown by the red arrow. By tuning the wavelength and angle of incidence, the point of zero reflection can be achieved because of the “topological protection”. Phase cannot be defined at the point of such complete darkness. However, at wavelengths close to this critical point, where the field intensity is still very small, sharp phase changes can be observed from the ellipsometric spectra. The experimental result for the setup in Figure 13B is reported in Figure 13C. The evolution of ellipsometric parameters, namely, the amplitude Ψ and phase Δ are plotted by the blue and red curves, respectively. The attachment of streptavidin molecules to nanodots causes a steep drop of phase by ∼25° within 2 min, which is much larger than the amplitude of the intensity change, promising an ultrasensitive realtime biomolecular recognition technique.
5.4 Chiral fields
Chiral metamaterials are another important branch of metamaterials, which are normally constructed from chiral elements, such as 3D metallic helices [10] and 2D gammadion unit cells [201] and spirals [202]. The unique structure of chiral metamaterials leads to a series of interesting phenomena with high chirality, for example, generating superchiral electromagnetic fields [203]. This characteristic provides a direct connection to bioapplications. It is well known that many building blocks of life comprise chiral molecular units, including amino acids and sugars. The biomacromolecules formed from these units inherit and exhibit chirality at the molecular and supramolecular level. Superchiral fields can offer a strong interaction with chiral materials with one or two orders of magnitude larger than that of circularly polarized waves used in traditional chiroptical methods. Hence, progress in chiral metamaterials may pave an avenue to ultrasensitive characterization of chiral molecules, which is beyond the conventional detection techniques such as circular dichroism (CD), optical rotatory dispersion, and Raman optical activity.
An experimental study based on planar chiral metamaterials (PCMs) has been reported in Ref. [174], which employs left and righthanded (LH/RH) gold gammadion arrays working at visible and nearinfrared frequencies. The gammadion units can induce local field enhancement that is always desired for achieving larger interaction with biomolecules and better sensitivity to dielectric environment changes. Three resonant modes in the gold gammadion arrays are observed from the CD spectra in Figure 14A. In addition, the excited localized SPPs in LH/RH gammadions behave differently and are coupled between branches to create strong field chirality. This character is also reflected in the plot. As one can see from Figure 14A, the spectrum of the LH gammadions is a perfect mirror image of that of the RH ones, implying a reversal of chirality of the generated field. When a biomacromolecule layer is adsorbed to the surface of PCMs, the property of the resonance shifts induced by refractive index change is determined by the chirality of the molecules and that of the fields. For an achiral adsorption such as ethanol, almost no shift is observed according to the first line in Figures 14B and 14C, where the scales of the bars are defined as the average and difference of the chiral resonance shifts in RH and LH PCMs, respectively. In sharp contrast, the behaviors of these two parameters are found to be quite different for chiral molecular layers. Specifically, large dissymmetry is observed in the difference of shifts on adsorption of tryptophan (negative) and βsheet proteins (positive), whereas the average shifts are larger for αhelical proteins. A special case is the heattreated βlactoglobulin. With the loss of βstructure at high temperature, the dissymmetry parameter exhibits a dramatic drop. The measurement results also provide indirect information about the geometry of the chiral molecules, which can be used to explain the different symmetric properties of the difference of resonance shifts. As can be seen in Figure 14D, biomacromolecules rich in αhelices (denoted by cyan cylinders) are more isotropically distributed at the interface with a relatively larger thickness, while the βsheet proteins (represented by ribbons) result in anisotropic aggregation in lateral directions but a thinner structure along the surface normal. It was previously revealed that the largest contributions of chiroptical phenomena come from the interactions of the electric dipolarmagnetic dipolar and the electric dipolarelectric quadrupolar excitations of molecules. The dipolar contributions always take effect in different media, but the quadrupolar contributions average to zero in isotropic materials [204]. As a result, when superchiral field is generated around the PCMs, the steep local field gradients can dramatically enhance the dipolequadrupole interactions over the dipoledipole ones in βsheet structures, leading to the large dissymmetries as in Figure 14C. Compared with schemes introduced in previous sections, a noticeable difference here is that the measurement process only relies on the RH and LH PCMs but does not need any recognition protein, which could lead to a feasible technique in ultrasensitive bioassaying.
Figure 14
6 Selfassembled plasmonic metamaterials
So far, various topdown fabrication methods, such as electron beam lithography, focused ion beam milling, direct laser writing, and nanoimprint lithography, have been applied to fabricate plasmonic and metamaterial structures. Both planar and 3D geometries with a feature size of sub100 nm can be reliably realized with high yield. However, it still remains challenging to achieve the spatial resolution smaller than 10 nm in welldefined architectures based on topdown processing. Meanwhile, the nonparallel procedures in topdown fabrications generally lead to long fabrication time. In comparison, selfassembly approach promises low cost, high efficiency, precise structural control at a truly nanometer scale, as well as sophisticated hierarchical structures with multifunction. Significant progress has been achieved in selfassembled plasmonic metamaterials in the past several years.
The study of nanoscale selfassembly of metallic nanoparticles started more than two decades ago. Nowadays, highquality metallic nanostructures with a variety of shapes (such as sphere, rod, cube, plate, pyramid, star, cage, coreshell, etc.) can be routinely achieved in the laboratory through optimized wet chemical synthesis techniques. As shown in Figure 15, the geometry, facet, or even inner structure of the nanoparticles could be rationally controlled, providing a complete, ingenious toolbox to construct complex metamaterials [205]. The interactions between nanoparticles, in addition to their size and shapes, play an important role in the resulting selfassembled geometry. These interactions include van der Waals forces, electrostatic forces, capillary forces, and molecular surface forces after decorating the surface of nanoparticles with various chemical functionalities [206, 207]. The magnitude and direction (i.e., attractive or repulsive) of these forces, as well as their working distances (i.e., long range or short range) are distinctly different. The intricate balance of these interactions gives rise to the spontaneous organization of nanoparticles into a relative stable structure at a thermodynamic equilibrium state, where the Gibbs free energy of the entire system is minimum. It should be noted that the interparticle forces at the nanoscale are still not fully understood, although we have achieved considerable advances in the area of selfassembly.
Figure 15
In 2010, Capasso’s group reported that selfassembled clusters of metaldielectric coreshell structures exhibit pronounced electric, magnetic, and Fano resonances, which can be readily tuned by adjusting the number and position of particles in the cluster [208]. The resonances of the clusters are attributed to the strong nearfield coupling between closely spaced particles, which can be described by plasmon hybridization [209, 210]. The building block of the clusters is goldsilica nano coreshell structures with tunable electric dipole resonance controlled by the coreshell aspect ratio. The spherical geometry supports orientationindependent coupling, ideal for constructing highly symmetric or isotropic metamaterials. Polymers with thiolated linkers in aqueous solutions are used to form monolayers on the surface of the coreshell nanoparticles. The polymer composition and chain length can be selected, leading to controllable gap size and optical coupling between nanoparticles. Finally, the polymercoated nanoshells are assembled into clusters by slowly drying a droplet of the coreshell nanoparticles on a hydrophobic substrate (Figure 16A). Darkfield spectroscopy is applied to measure the intriguing optical properties of individual nanoshell clusters. For instance, a trimer, consisting of three coreshell nanoparticles, supports a magnetic dipole mode that originates from the induced inplane current loop. In the experiment, a crosspolarizer is used with spolarized incident light to filter out the scattered electric dipole radiation. This scheme is particularly useful for detecting the magnetic dipole mode that can be obscured by the broad electric dipole peak in scattering spectra. As shown in Figure 16B, the peak around 1400 nm corresponds to the magnetic dipole mode. The magnetic dipole mode exhibits a sharper spectral width and a red shift in comparison to the electric dipole mode, in good agreement with the simulation result. A 3D tetrahedral cluster can support isotropic magnetic resonances. Furthermore, Fano resonance is observed in a heptamer plasmonic cluster that is composed of seven identical elements. The overall dipole moment of the outer hexagon is similar in magnitude but opposite in sign with respect to the dipole moment of the central coreshell nanoparticle, leading to strong destructive interference of their radiating fields and the asymmetric line shape.
Figure 16
DNAguided assembly is an alternative, viable method for controllable arrangement of nanoparticles of different size and composition [205]. The unique and specific WatsonCrick base pairing of DNA, that is, adeninethymine (AT) and guaninecytosine (GC), offers systematically and precisely programmable hydrogen bonding. The length and the mechanical strength of DNA strands can be finely and widely tuned over a large range. All of these merits enable DNA as a superior interface to regulate the interactions between nanoparticles and produce desired selfassembly hierarchy with judicious structural and sequence design. The recently developed DNAorigami technique even allows pattern designs in an almost arbitrary manner [212]. The key is to use specific short singlestranded DNA as “staple” to direct the folding of a long single strand into the desired shape.
Utilizing DNA as a ligand through monofunctionalization and anisotropic functionalization, a vast assortment of plasmonic molecules and crystals has been realized. For example, the seminal work has shown that singlestranded DNA (ssDNA) can be attached to gold nanoparticles via a thiol linker, and subsequently, nanoparticles are assembled by the hybridization of the DNA into a double helix [213, 214]. A doublestranded DNA pyramidal scaffold is capable of controlling the position and arrangement of gold nanoparticles, resulting in discrete, tetrahedral nanostructures [215]. Such a tetrahedral plasmonic “molecule” exhibits strong chiral optical properties. Anisotropic functionalization provides another route to generate a diverse selection of discrete plasmonic molecules, in which the size and composition of individual nanoparticles could be varied [216, 217]. DNA origami probably represents the ultimate solution for programmable and nanometerprecise design of plasmonic metamaterials. Using this technique, Kuzyk and coworkers fabricated chiral plasmonic nanostructures showing strong circular dichroism at visible wavelengths [211]. Figure 16C is the schematic illustration of the design. Left and righthanded nanohelices (helical pitch 57 nm) are formed by attaching nine gold nanoparticles (diameter 10 nm) to the surface of DNA origami 24helix bundles (diameter 16 nm). Each of the nine attachment sites consists of three singlestranded extensions of staple oligonucleotides. Gold nanoparticles are coated with multiple thiolmodified DNA strands, which are complementary to these staple extensions. The mixture of gold nanoparticles and 24helix bundles will, hence, result in the designed plasmonic helical structures. Owing to their intrinsic geometric handness, lefthanded and righthanded helices respond to leftcircularly and rightcircularly polarized light differently. The CD spectra, i.e., the differential absorption of left/right circularly polarized light, are plotted in Figure 16D. The characteristic bisignate peakdip line shapes, which are vertically mirrored for the two helical structures, agree well with theoretical calculations in terms of the spectral wavelength and signal strength. The CD signal can be further enhanced when nanoparticles are larger or arranged in a smaller helical pitch.
In terms of largearea selfassembled plasmonic metamaterials, different approaches have been proposed and demonstrated [218–221]. For example, Gwo’s group reported a simple method for synthesizing 3D plasmonic crystals over an area >1 cm^{2} consisting of gold and silver nanoparticles (Figure 17A–D) [222]. In their experiments, Janus nanoparticles, which have solventphobic top surface and solventphilic bottom surface, form closepacked monolayers based on layerbylayer (LbL) assembly from suspensions of thiolatepassivated gold or silver colloids. Such plasmonic crystals exhibit strong transverse (intralayer) and longitudinal (interlayer) nearfiled coupling. Furthermore, largearea superlattices with two or three types of nanostructures promise a new route for designing metamaterials with rationally tunable properties by adjusting the chemical composition, size, and stoichiometry of the constituents [225, 226]. Dong et al. recently demonstrated the selfassembly and transfer of macroscopic, longrangeordered supperlattices made of binary or trinary nanocrystals using the liquidair interfacial assembly approach (Figure 17E and F) [223, 227]. New synthetic methods result in monodisperse Ag nanocrystals with welldefined polyhedral shapes, including cubes, truncated cubes, cuboctahedra, octahedra, and truncated octahedra [228]. The particle shape provides an additional handle to twist the structure of assembled patterns, when the polyhedra are selfassembled into longrange ordered superstructures. In one experiment, monodisperse Ag polyhedra, coated with polyvinylpyrrolidone (PVP), assemble into large, dense supercrystals by gravitational sedimentation [224]. Unlike cubes and truncated octahedra, octahedra in their densest lattice packing show only incomplete facetoface contact, and the equivalent faces of neighboring octahedra either do not lie in a common plane. Unadsorbed PVP polymer in solution will induce attractions between particles, leading to new structures that are not governed solely by packing efficiency of hard shapes. As shown in Figure 17G and H, a lattice of octahedra with intriguing helical motifs is generated, if extra PVP is added to the solution immediately before sedimentation. Higher amounts of PVP result in less Minkowski lattice and more helical lattice. This characteristic is confirmed by Monte Carlo simulation (Figure 17I). The large degree of facetoface contact in the latter reflects significant attractive forces.
Figure 17
7 Conclusion and outlook
We have seen rapid growth in the field of plasmonic metamaterials, and it will continuously advance. The integration of plasmonics and metamaterials results in several benefits, rendering plasmonic metamaterials a promising platform to explore complex optical effects and new applications. First, the large local field enhancement leads to stronger lightmatter interaction, through which many weak processes can be enhanced and effectively utilized. Second, the tight field confinement and ultrafast optical process enable the construction of miniaturized devices, working either as the bridge of photonic and electronic components, or even alloptical photonic circuits. Third, the spectra of plasmonic metamaterials are highly tunable by altering the responses of individual constituents and their coupling. This is highly desirable in almost all the practical situations. Owing to these attractive features, plasmonic metamaterials are expected to extend to a much broader horizon beyond what we have discussed in this review article. We think that the following areas are still largely unexplored, and worth to devote special efforts.

The first one is nonlinear optics in plasmonic metamaterials. The large local field can provide strongly enhanced nonlinear processes, if we embed nonlinear materials into plasmonic nanostructures. In addition, the metal itself has high intrinsic nonlinearity, which can be further amplified by texturing the metal surface. An enhancement of four orders of magnitude in conversion efficiency for optical secondharmonic generation has been experimentally demonstrated in a periodically nanostructured metal structure [229]. Very recently, up to the 43rd harmonic generation of ultrashort extremeultraviolet pulses have been achieved by means of the plasmonic field enhancement [230, 231]. It is shown that the strong magnetic resonance, whose contribution is normally ignored, could substantially modify the nonlinear optical process [232, 233]. In terms of negative refraction, an alternative approach based on phase conjugation from a thin nonlinear film has been proposed [234, 235]. Such a scheme was experimentally demonstrated in the microwave region [236] and at optical frequencies using fourwave mixing in nanostructured metal films [237] and graphite thin films [238], respectively. Other intriguing nonlinear phenomena, such as unusual phase matching [239, 240] and solitary wave propagation [241, 242] are worth for experimental exploration. All of these exciting phenomena and developments promise tunable metamaterials, ultrafast switching, and optical modulation [243–246].

There is an explosively growing interest in expanding the properties of plasmonics and metamaterials toward the quantum regime and studying how plasmonics and metamaterials can mediate lightmatter interaction with new functionalities at the nanoscale [247]. For example, researchers have demonstrated the survival of photon entanglement in plasmonic systems [248], the blue shift and linewidth broadening of the plasmon resonance due to the quantum size effect [249, 250], and electron tunneling between two nanoparticles with a separation distance less than 1 nm [251, 252]. New theories based on the nonlocality [253, 254] and the quantumcorrected model [255] have also been developed to study the plasmonic field enhancement at such extremely small scales. In addition, the large photonic density of states in hyperbolic metamaterials is able to increase the interaction with the quantum emitter while simultaneously channeling the light into a subdiffraction singlephoton resonance cone [256]. The research outcome in the new frontier of quantum plasmonics and quantum metamaterials will considerably advance our understanding of the fundamental physics associated with SPPs and metamaterials and facilitate the development of novel quantum photonic and electronic components [257–261] including singlephoton sources, nanoscale lasers, transistors, and detectors.

Dynamically reconfigurable plasmonic metamaterials is also a valuable subject to explore. Although the modulation of subwavelength features at optical regime is challenging, significant advancement has been achieved to overcome this obstacle. The usage of graphene, phasechange media [262, 263], liquid metals [264], or liquid crystals [265, 266] provides possible solutions from the material aspect, and electrical modulation of structural patterns [267] and MEMS [268, 269] solves the problem from the structure aspect. In particular, plasmonic metamaterials operating in the fluidic environment may realize the ultimate reconfigurability and multiple functionalities. Very recently, laserinduced surface bubbles are used to manipulate the propagation of SPPs. By precisely controlling the size, location, and shape of the surface bubbles, as well as the phase front of the incident SPPs, divergence, collimation, and focusing of SPPs are all obtained by such plasmofluidic lenses [270]. Moreover, molecularcontrolled nanoparticle assembly in solutions has been successfully demonstrated, providing a powerful building block of plasmonic metamaterials at deep subwavelength scale.
In conclusion, we have witnessed tremendous progress of metamaterials and plasmonics over the past decade. The alliance of metamaterials and plasmonics will inevitably offer novel opportunities to advance both fields and stimulate new crossdisciplinary approaches to address grand challenges in information processing, clean energy, and human health. Many important discoveries and applications in the emerging field of plasmonic metamaterials are awaiting us to exploit.
References
[1] Smith D, Pendry J, Wiltshire M. Metamaterials and negative refractive index. Science 2004, 305, 788–792. Search in Google Scholar
[2] Liu Y, Zhang X. Metamaterials: a new frontier of science and technology. Chem. Soc. Rev. 2011, 40, 2494–2507. Search in Google Scholar
[3] Soukoulis CM, Wegener M. Past achievements and future challenges in the development of threedimensional photonic metamaterials. Nat. Photonics 2011, 5, 523–530. Search in Google Scholar
[4] Cai W, Shalaev VM. Optical Metamaterials: Fundamentals and Applications, Springer: New York, 2010. Search in Google Scholar
[5] Smith D, Schultz S, Markoš P, Soukoulis C. Determination of effective permittivity and permeability of metamaterials from reflection and transmission coefficients. Phys. Rev. B 2002, 65, 195104. Search in Google Scholar
[6] Pendry JB, Holden A, Stewart W, Youngs I. Extremely low frequency plasmons in metallic mesostructures. Phys. Rev. Lett. 1996, 76, 4773–4776. Search in Google Scholar
[7] Pendry JB, Holden A, Robbins D, Stewart W. Magnetism from conductors and enhanced nonlinear phenomena. IEEE Trans. Microw. Theory Tech. 1999, 47, 2075–2084. Search in Google Scholar
[8] Smith DR, Kroll N. Negative refractive index in lefthanded materials. Phys. Rev. Lett. 2000, 85, 2933–2936. Search in Google Scholar
[9] Choi M, Lee SH, Kim Y, Kang SB, Shin J, Kwak MH, Kang KY, Lee YH, Park N, Min B. A terahertz metamaterial with unnaturally high refractive index. Nature 2011, 470, 369–373. Search in Google Scholar
[10] Gansel JK, Thiel M, Rill MS, Decker M, Bade K, Saile V, Freymann GV, Linden S, Wegener M. Gold helix photonic metamaterial as broadband circular polarizer. Science 2009, 325, 1513–1515. Search in Google Scholar
[11] Pendry JB, Schurig D, Smith DR. Controlling electromagnetic fields. Science 2006, 312, 1780–1782. Search in Google Scholar
[12] Leonhardt U. Optical conformal mapping. Science 2006, 312, 1777–1780. Search in Google Scholar
[13] Greenleaf A, Kurylev Y, Lassas M, Uhlmann G. Cloaking devices, electromagnetic wormholes, and transformation optics. SIAM Rev. 2009, 51, 3–33. Search in Google Scholar
[14] Chen H, Chan C, Sheng P. Transformation optics and metamaterials. Nat. Mater. 2010, 9, 387–396. Search in Google Scholar
[15] Liu Y, Zhang X. Recent advances in transformation optics. Nanoscale 2012, 4, 5277–5292. Search in Google Scholar
[16] Soukoulis CM. Negative refractive index at optical wavelengths. Science 2007, 315, 47–49. Search in Google Scholar
[17] Klein M, Enkrich C, Wegener M, Soukoulis C, Linden S. Singleslit splitring resonators at optical frequencies: limits of size scaling. Opt. Lett. 2006, 31, 1259–1261. Search in Google Scholar
[18] Zhou J, Koschny Th, Kafesaki M, Economou EN, Pendry JB, Soukoulis CM. Saturation of the magnetic response of splitring resonators at optical frequencies. Phys. Rev. Lett. 2005, 95, 223902. Search in Google Scholar
[19] Tretyakov S. On geometrical scaling of splitring and doublebar resonators at optical frequencies. Metamaterials 2007, 1, 40–43. Search in Google Scholar
[20] Raether, H. Surface Plasmons, SpringerVerlag: Berlin, 1988. Search in Google Scholar
[21] Maier SA. Plasmonics: Fundamentals and Applications, Springer Science+Business Media: New York, 2007. Search in Google Scholar
[22] Anker JN, Hall WP, Lyandres O, Shah NC, Zhao J, Van Duyne RP. Biosensing with plasmonic nanosensors. Nat. Mater. 2008, 7, 442–453. Search in Google Scholar
[23] Zhang X, Liu, Z. Superlenses to overcome the diffraction limit. Nat. Mater. 2008, 7, 435–441. Search in Google Scholar
[24] Atwater HA, Polman A. Plasmonics for improved photovoltaic devices. Nat. Mater. 2010, 9, 205–213. Search in Google Scholar
[25] Srituravanich W, Fang N, Sun C, Luo Q, Zhang X. Plasmonic nanolithography. Nano Lett. 2004, 4, 1085–1088. Search in Google Scholar
[26] Gramotnev DK, Bozhevolnyi SI. Plasmonics beyond the diffraction limit. Nat. Photonics 2010, 4, 83–91. Search in Google Scholar
[27] Chaturvedi P, Wu W, Logeeswaran VJ, Yu Z, Islam S, Wang SY, Williams RS, Fang NX. A smooth optical superlens. Appl. Phys. Lett. 2010, 96, 043102. Search in Google Scholar
[28] Nie S, Emory SR. Probing single molecules and single nanoparticles by surfaceenhanced Raman scattering. Science 1997, 275, 1102–1106. Search in Google Scholar
[29] Kneipp K, Wang Y, Kneipp H, Perelman LT, Itzkan I, Dasari RR, Feld MS. Single molecule detection using surfaceenhanced Raman scattering (SERS). Phys. Rev. Lett. 1997, 78, 1667. Search in Google Scholar
[30] Campion A, Kambhampati P. Surfaceenhanced Raman scattering. Chem. Soc. Rev. 1998, 27, 241–250. Search in Google Scholar
[31] Zhang R, Zhang Y, Dong ZC, Jiang S, Zhang C, Chen LG, Zhang L, Liao Y, Aizpurua J, Luo Y, Yang JL, Hou JG. Chemical mapping of a single molecule by plasmonenhanced Raman scattering. Nature 2013, 498, 82–86. Search in Google Scholar
[32] Veselago VG. The electrodynamics of substances with simultaneously negative values of ε and μ. PhysicsUspekhi 1968, 10, 509–514. Search in Google Scholar
[33] Shelby R, Smith D, Schultz S. Experimental verification of a negative index of refraction. Science 2001, 292, 77–79. Search in Google Scholar
[34] Valentine J, Zhang S, Zentgraf T, UlinAvila E, Genov DA, Bartal G, Zhang X. Threedimensional optical metamaterial with a negative refractive index. Nature 2008, 455, 376–379. Search in Google Scholar
[35] Zhang S, Fan W, Panoiu NC, Malloy KJ, Osgood RM, Brueck SRJ. Experimental demonstration of nearinfrared negativeindex metamaterials. Phys. Rev. Lett. 2005, 95, 137404. Search in Google Scholar
[36] Xiao S, Drachev VP, Kildishev AV, Ni X, Chettiar UK, Yuan HK, Shalaev VM. Lossfree and active optical negativeindex metamaterials. Nature 2010, 466, 735–738. Search in Google Scholar
[37] Shin H, Fan S. Allangle negative refraction for surface plasmon waves using a metaldielectricmetal structure. Phys. Rev. Lett. 2006, 96, 073907. Search in Google Scholar
[38] Lezec HJ, Dionne JA, Atwater HA. Negative refraction at visible frequencies. Science 2007, 316, 430–432. Search in Google Scholar
[39] Verhagen E, de Waele R, Kuipers L, Polman A. Threedimensional negative index of refraction at optical frequencies by coupling plasmonic waveguides. Phys. Rev. Lett. 2010, 105, 223901. Search in Google Scholar
[40] Burgos SP, de Waele R, Polman A, Atwater HA. A singlelayer wideangle negativeindex metamaterial at visible frequencies. Nat. Mater. 2010, 9, 407–412. Search in Google Scholar
[41] Xu T, Agrawal A, Abashin M, Chau KJ, Lezec HJ. Allangle negative refraction and active flat lensing of ultraviolet light. Nature 2013, 497, 470–474. Search in Google Scholar
[42] Atre AC, GarcíaEtxarri A, Alaeian H, Dionne JA. A broadband negative index metamaterial at optical frequencies. Adv. Opt. Mater. 2013, 1, 327–333. Search in Google Scholar
[43] Vesseur EJR, Coenen T, Caglayan H, Engheta N, Polman A. Experimental verification of n=0 structures for visible light. Phys. Rev. Lett. 2013, 110, 013902. Search in Google Scholar
[44] Yao J, Liu Z, Liu Y, Wang Y, Sun C, Bartal G, Stacy AM, Zhang X. Optical negative refraction in bulk metamaterials of nanowires. Science 2008, 321, 930–930. Search in Google Scholar
[45] Liu Y, Bartal G, Zhang X. Allangle negative refraction and imaging in a bulk medium made of metallic nanowires in the visible region. Opt. Exp. 2008, 16, 15439–15448. Search in Google Scholar
[46] Fang A, Koschny T, Soukoulis CM. Optical anisotropic metamaterials: negative refraction and focusing. Phys. Rev. B 2009, 79, 245127. Search in Google Scholar
[47] Wheeler MS, Aitchison JS, Mojahedi M. Threedimensional array of dielectric spheres with an isotropic negative permeability at infrared frequencies. Phys. Rev. B 2005, 72, 193103. Search in Google Scholar
[48] Vynck K, Felbacq D, Centeno E, Cabuz AI, Cassagne D, Guizal B. Alldielectric rodtype metamaterials at optical frequencies. Phys. Rev. Lett. 2009, 102, 133901. Search in Google Scholar
[49] Schuller JA, Zia R, Taubner T, Brongersma ML. Dielectric metamaterials based on electric and magnetic resonances of silicon carbide particles. Phys. Rev. Lett. 2007, 99, 107401. Search in Google Scholar
[50] Simovski C, Tretyakov S. Model of isotropic resonant magnetism in the visible range based on coreshell clusters. Phys. Rev. B 2009, 79, 045111. Search in Google Scholar
[51] PaniaguaDomínguez R, LópezTejeira F, Marqués R, SánchezGil JA. Metallodielectric core–shell nanospheres as building blocks for optical threedimensional isotropic negativeindex metamaterials. New J. Phys. 2011, 13, 123017. Search in Google Scholar
[52] PaniaguaDomínguez R, Abujetas D, SánchezGil J. Ultra lowloss, isotropic optical negativeindex metamaterial based on hybrid metalsemiconductor nanowires. Sci. Rep. 2013, 3, 1507. Search in Google Scholar
[53] Muhlig S, Cunningham A, Scheeler S, Pacholski C, Bürgi T, Rockstuh C, Lederer F. Selfassembled plasmonic coreshell clusters with an isotropic magnetic dipole response in the visible range. ACS Nano 2011, 5, 6586–6592. Search in Google Scholar
[54] Čerenkov P. Visible radiation produced by electrons moving in a medium with velocities exceeding that of light. Phys. Rev. 1937, 52, 378–379. Search in Google Scholar
[55] Chen H, Chen M. Flipping photons backward: reversed Cherenkov radiation. Mater. Today 2011, 14, 34–41. Search in Google Scholar
[56] Zhang S, Zhang X. Flipping a photonic shock wave. Physics 2009, 2, 91. Search in Google Scholar
[57] Xi S, Chen H, Jiang T, Ran L, Huangfu J, Wu BI, Kong JA, Chen M. Experimental verification of reversed Cherenkov radiation in lefthanded metamaterial. Phys. Rev. Lett. 2009, 103, 194801. Search in Google Scholar
[58] Grbic A, Eleftheriades GV. Experimental verification of backwardwave radiation from a negative refractive index metamaterial. J. Appl. Phys. 2002, 92, 5930–5935. Search in Google Scholar
[59] Antipov S, Spentzouris L, Gai W, Conde M, Franchini F, Konecny R, Liu W, Power JG, Yusof Z, Jing C. Observation of wakefield generation in lefthanded band of metamaterialloaded waveguide. J. Appl. Phys. 2008, 104, 014901. Search in Google Scholar
[60] Seddon N, Bearpark T. Observation of the inverse Doppler effect. Science 2003, 302, 1537–1540. Search in Google Scholar
[61] Chen J, Wang Y, Jia B, Geng T, Li X, Feng L, Qian W, Liang B, Zhang X, Gu M, Zhuang S. Observation of the inverse Doppler effect in negativeindex materials at optical frequencies. Nat. Photonics 2011, 5, 239–245. Search in Google Scholar
[62] Kemp BA, Kong JA, Grzegorczyk TM. Reversal of wave momentum in isotropic lefthanded media. Phys. Rev. A 2007, 75, 053810. Search in Google Scholar
[63] Minkowski H. Die Grundgleichungen für die elektromagnetischen Vorgänge in bewegten Körpern. Nachr. Ges. Wiss. Göttingen, Math.Phys. Kl. 1908, 1908, 53–111. Search in Google Scholar
[64] Abraham M. Zur elektrodynamik bewegter körper. Rend. Circ. Mat. Palermo (1884–1940) 1909, 28, 1–28. Search in Google Scholar
[65] Leonhardt U. Momentum in an uncertain light. Nature 2006, 444, 823–824. Search in Google Scholar
[66] Veselago VG. Energy, linear momentum and mass transfer by an electromagnetic wave in a negativerefraction medium. Phys.Usp. 2009, 52, 649–654. Search in Google Scholar
[67] Chau KJ, Lezec HJ. Revisiting the Balazs thought experiment in the case of a lefthanded material: electromagneticpulseinduced displacement of a dispersive, dissipative negativeindex slab. Opt. Exp. 2012, 20, 10138–10162. Search in Google Scholar
[68] Mansuripur M, Zakharian AR. Radiation pressure and photon momentum in negativeindex media. Proc. SPIE 2012, 8455, 845511. Search in Google Scholar
[69] Nemirovsky J, Rechtsman MC, Segev M. Negative radiation pressure and negative effective refractive index via dielectric birefringence. Opt. Exp. 2012, 20, 8907–8914. Search in Google Scholar
[70] Chen J, Ng J, Lin Z, Chan CT. Optical pulling force. Nat. Photonics 2011, 5, 531–534. Search in Google Scholar
[71] Sukhov S, Dogariu A. Negative nonconservative forces: optical “tractor beams” for arbitrary objects. Phys. Rev. Lett. 2011, 107, 203602. Search in Google Scholar
[72] Kajorndejnukul V, Ding W, Sukhov S, Qiu CW, Dogariu A. Linear momentum increase and negative optical forces at dielectric interface. Nat. Photonics 2013, 7, 787–790. Search in Google Scholar
[73] Dogariu A, Sukhov S, Sáenz J. Optically induced ‘negative forces’. Nat. Photonics 2012, 7, 24–27. Search in Google Scholar
[74] Yu N, Genevet P, Kats MA, Aieta F, Tetienne JP, Capasso F, Gaburro Z. Light propagation with phase discontinuities: generalized laws of reflection and refraction. Science 2011, 334, 333–337. Search in Google Scholar
[75] Ni X, Emani NK, Kildishev AV, Boltasseva A, Shalaev VM. Broadband light bending with plasmonic nanoantennas. Science 2012, 335, 427. Search in Google Scholar
[76] Sun S, He Q, Xiao S, Xu Q, Li X, Zhou L. Gradientindex metasurfaces as a bridge linking propagating waves and surface waves. Nat. Mater. 2012, 11, 426–431. Search in Google Scholar
[77] Kildishev AV, Boltasseva A, Shalaev VM. Planar photonics with metasurfaces. Science 2013, 339, 6125. Search in Google Scholar
[78] Yin X, Ye Z, Rho J, Wang Y, Zhang X. Photonic spin Hall effect at metasurfaces. Science 2013, 339, 1405–1407. Search in Google Scholar
[79] Lin J, Mueller JPB, Wang Q, Yuan G, Antoniou N, Yuan XC, Capasso F. Polarizationcontrolled tunable directional coupling of surface plasmon polaritons. Science 2013, 340, 331–334. Search in Google Scholar
[80] RodríguezFortuño FJ, Marino G, Ginzburg P, O’Connor D, Martínez A, Wurtz GA, Zayats AV. Nearfield interference for the unidirectional excitation of electromagnetic guided modes. Science 2013, 340, 328–330. Search in Google Scholar
[81] Huang L, Chen X, Bai B, Tan Q, Jin G, Zentgraf T, Zhang S. Helicity dependent directional surface plasmon polariton excitation using a metasurface with interfacial phase discontinuity. Light Sci. Appl. 2013, 2, e70. Search in Google Scholar
[82] Shitrit N, Yulevich I, Maguid E, Ozeri D, Veksler D, Kleiner V, Hasman E. Spinoptical metamaterial route to spincontrolled photonics. Science 2013, 340, 724–726. Search in Google Scholar
[83] Grady NK, Heyes JE, Chowdhury DR, Zeng Y, Reiten MT, Azad AK, Taylor AT, Dalvit DAR, Chen HT. Terahertz metamaterials for linear polarization conversion and anomalous refraction. Science 2013, 340, 1304–1307. Search in Google Scholar
[84] Chen X, Huang L, Mühlenbernd H, Li G, Bai B, Tan Q, Jin G, Qiu CH, Zhang S, Zentgraf T. Dualpolarity plasmonic metalens for visible light. Nat. Commun. 2012, 3, 1198. Search in Google Scholar
[85] Moreau A, Ciracì C, Mock JJ, Hill RT, Wang Q, Wiley BJ, Chilkoti A, Smith DR. Controlledreflectance surfaces with filmcoupled colloidal nanoantennas. Nature 2012, 492, 86–89. Search in Google Scholar
[86] Munk BA. Frequency Selective Surfaces: Theory and Design, John Wiley & Sons: New York, 2000. Search in Google Scholar
[87] Ryan CG, Mil R, Chaharmir MR, Shaker J, Bray JR. A wideband transmitarray using dualresonant double square rings. IEEE Trans.Antennas Propag. 2010, 58, 1486–1493. Search in Google Scholar
[88] Sazegar M, Zheng Y, Maune H, Nikfalazar M, Jakoby, R. Beam steering transmitarray using a tunable frequency selective surface with integrated ferroelectric varactors. IEEE Trans.Antennas Propag. 2012, 60, 5690–5699. Search in Google Scholar
[89] Pozar DM, Targonski SD, Syrigos H. Design of millimeter wave microstrip reflectarrays. IEEE Trans.Antennas Propag. 1997, 45, 287–296. Search in Google Scholar
[90] Costa F, Monorchio A, Manara G. Analysis and design of ultra thin electromagnetic absorbers comprising resistively loaded high impedance surfaces. IEEE Trans.Antennas Propag. 2010, 58, 1551–1558. Search in Google Scholar
[91] Sun J, Timurdogan E, Yaacobi A, Hosseini ES, Watts MR. Largescale nanophotonic phased array. Nature 2013, 493, 195–199. Search in Google Scholar
[92] Aieta F, Genevet P, Yu N, Kats MA, Gaburro Z, Capasso F. Outofplane reflection and refraction of light by anisotropic optical antenna metasurfaces with phase discontinuities. Nano Lett. 2012, 12, 1702–1706. Search in Google Scholar
[93] Aieta F, Genevet P, Kats MA, Yu N, Blanchard R, Gaburro Z, Capasso F. Aberrationfree ultrathin flat lenses and axicons at telecom wavelengths based on plasmonic metasurfaces. Nano Lett. 2012, 12, 4932–4936. Search in Google Scholar
[94] Huang L, Chen X, Mühlenbernd H, Li G, Bai B, Tan Q, Jin G, Zentgraf T, Zhang S. Dispersionless phase discontinuities for controlling light propagation. Nano Lett. 2012, 12, 5750–5755. Search in Google Scholar
[95] Yu N, Aieta F, Genevet P, Kats MA, Gaburro Z, Capasso F. A broadband, backgroundfree quarterwave plate based on plasmonic metasurfaces. Nano Lett. 2012, 12, 6328–6333. Search in Google Scholar
[96] Pors A, Nielsen MG, Eriksen RL, Bozhevolnyi SI. Broadband focusing flat mirrors based on plasmonic gradient metasurfaces. Nano Lett. 2013, 13, 829–834. Search in Google Scholar
[97] Walther B, Helgert C, Rockstuh C, Setzpfandt F, Eilenberger F, Kley EB, Lederer F, Tünnermann A, Pertsch T. Spatial and spectral light shaping with metamaterials. Adv. Mater. 2012, 24, 6300–6304. Search in Google Scholar
[98] Kats MA, Genevet P, Aoust G, Yu N, Blanchard R, Aieta F, Gaburro Z, Capasso F. Giant birefringence in optical antenna arrays with widely tailorable optical anisotropy. Proc. Natl. Acad. Sci. USA 2012, 109, 12364–12368. Search in Google Scholar
[99] Pors A, Albrektsen O, Radko IP, Bozhevolnyi SI. Gap plasmonbased metasurfaces for total control of reflected light. Sci. Rep. 2013, 3, 2155. Search in Google Scholar
[100] Lavery MPJ, Speirits FC, Barnett SM, Padgett MJ. Detection of a spinning object using light’s orbital angular momentum. Science 2013, 341, 537–540. Search in Google Scholar
[101] Curtis JE, Koss BA, Grier DG. Dynamic holographic optical tweezers. Opt. Commun. 2002, 207, 169–175. Search in Google Scholar
[102] Grier DG. A revolution in optical manipulation. Nature 2003, 424, 810–816. Search in Google Scholar
[103] Gibson G, Courtial J, Padgett MJ, Vasnetsov M, Pas’ko V, Barnett SM, FrankeArnold S. Freespace information transfer using light beams carrying orbital angular momentum. Opt. Exp. 2004, 12, 5448–5456. Search in Google Scholar
[104] Barreiro JT, Wei TC, Kwiat PG. Beating the channel capacity limit for linear photonic superdense coding. Nat. Phys. 2008, 4, 282–286. Search in Google Scholar
[105] Allen L, Beijersbergen M, Spreeuw R, Woerdman J. Orbital angular momentum of light and the transformation of LaguerreGaussian laser modes. Phys. Rev. A 1992, 45, 8185–8189. Search in Google Scholar
[106] Marrucci L, Manzo C, Paparo D. Optical spintoorbital angular momentum conversion in inhomogeneous anisotropic media. Phys. Rev. Lett. 2006, 96, 163905. Search in Google Scholar
[107] Bliokh KY, Niv A, Kleiner V, Hasman E. Geometrodynamics of spinning light. Nat. Photonics 2008, 2, 748–753. Search in Google Scholar
[108] Wunderlich J, Kaestner B, Sinova J, Jungwirth T. Experimental observation of the spinHall effect in a twodimensional spinorbit coupled semiconductor system. Phys. Rev. Lett. 2005, 94, 047204. Search in Google Scholar
[109] Hosten O, Kwiat P. Observation of the spin Hall effect of light via weak measurements. Science 2008, 319, 787–790. Search in Google Scholar
[110] Leyder C, Romanelli M, Karr JPh, Giacobino E, Liew TCH, Glazov MM, Kavokin AV, Malpuech G, Bramati A. Observation of the optical spin Hall effect. Nat. Phys. 2007, 3, 628–631. Search in Google Scholar
[111] Lu D, Liu Z. Hyperlenses and metalenses for farfield superresolution imaging. Nat. Commun. 2012, 3, 1205. Search in Google Scholar
[112] Pfeiffer C, Grbic A. Metamaterial Huygens’ surfaces: tailoring wave fronts with reflectionless sheets. Phys. Rev. Lett. 2013, 110, 197401. Search in Google Scholar
[113] Monticone F, Estakhri NM, Alù A. Full control of nanoscale optical transmission with a composite metascreen. Phys. Rev. Lett. 2013, 110, 203903. Search in Google Scholar
[114] Liu Y, Zentgraf T, Bartal G, Zhang, X. Transformational plasmon optics. Nano Lett. 2010, 10, 1991–1997. Search in Google Scholar
[115] Huidobro PA, Nesterov ML, MartínMoreno L, GarcíaVidal FJ. Transformation optics for plasmonics. Nano Lett. 2010, 10, 1985–1990. Search in Google Scholar
[116] Aubry A, Lei DY, FernándezDomínguez AI, Sonnefraud Y, Maier SA, Pendry JB. Plasmonic lightharvesting devices over the whole visible spectrum. Nano Lett. 2010, 10, 2574–2579. Search in Google Scholar
[117] Liu Y, Palomba S, Park Y, Zentgraf T, Yin X, Zhang X. Compact magnetic antennas for directional excitation of surface plasmons. Nano Lett. 2012, 12, 4853–4858. Search in Google Scholar
[118] Liu Y, Zhang X. Metasurfaces for manipulating surface plasmons. Appl. Phys. Lett. 2013, 103, 141101. Search in Google Scholar
[119] Novoselov KS, Geim AK, Morozov SV, Jiang D, Zhang Y, Dubonos SV, Grigorieva IV, Firsov AA. Electric field effect in atomically thin carbon films. Science 2004, 306, 666–669. Search in Google Scholar
[120] Novoselov K, Jiang D, Schedin F, Booth TJ, Khotkevich VV, Morozov SV, Geim AK. Twodimensional atomic crystals. Proc. Natl. Acad. Sci. USA 2005, 102, 10451–10453. Search in Google Scholar
[121] Grigorenko A, Polini M, Novoselov K. Graphene plasmonics. Nat. Photonics 2012, 6, 749–758. Search in Google Scholar
[122] Rana F. Graphene terahertz plasmon oscillators. IEEE Trans. Nanotechnol. 2008, 7, 91–99. Search in Google Scholar
[123] Jablan M, Buljan H, Soljačić M. Plasmonics in graphene at infrared frequencies. Phys. Rev. B 2009, 80, 245435. Search in Google Scholar
[124] Koppens FH, Chang DE, Garcia de Abajo FJ. Graphene plasmonics: a platform for strong lightmatter interactions. Nano Lett. 2011, 11, 3370–3377. Search in Google Scholar
[125] Vakil A, Engheta N. Transformation optics using graphene. Science 2011, 332, 1291–1294. Search in Google Scholar
[126] Bao Q, Loh KP. Graphene photonics, plasmonics, and broadband optoelectronic devices. ACS Nano 2012, 6, 3677–3694. Search in Google Scholar
[127] Tassin P, Koschny T, Kafesaki M, Soukoulis CM. A comparison of graphene, superconductors and metals as conductors for metamaterials and plasmonics. Nat. Photonics 2012, 6, 259–264. Search in Google Scholar
[128] Neto AC, Guinea F, Peres N, Novoselov KS, Geim AK. The electronic properties of graphene. Rev. Modern Phys. 2009, 81, 109–162. Search in Google Scholar
[129] Wang F, Zhang Y, Tian C, Girit C, Zettl A, Crommie M, Shen YR. Gatevariable optical transitions in graphene. Science 2008, 320, 206–209. Search in Google Scholar
[130] Li Z, Henriksen EA, Jiang Z, Hao Z, Martin MC, Kim P, Stormer HL, Basov DN. Dirac charge dynamics in graphene by infrared spectroscopy. Nat. Phys. 2008, 4, 532–535. Search in Google Scholar
[131] Mak KF, Sfeir MY, Wu Y, Lui CH, Misewich JA, Heinz TF. Measurement of the optical conductivity of graphene. Phys. Rev. Lett. 2008, 101, 196405. Search in Google Scholar
[132] Giovannetti G, Khomyakov PA, Brocks G, Karpan VM, Brink VD, Kelly PJ. Doping graphene with metal contacts. Phys. Rev. Lett. 2008, 101, 026803. Search in Google Scholar
[133] Zhang Y, Tang TT, Girit C, Hao Z, Martin MC, Zettl A, Crommie MF, Shen RY, Wang F. Direct observation of a widely tunable bandgap in bilayer graphene. Nature 2009, 459, 820–823. Search in Google Scholar
[134] Bonaccorso F, Sun Z, Hasan T, Ferrari A. Graphene photonics and optoelectronics. Nat. Photonics 2010, 4, 611–622. Search in Google Scholar
[135] Fei Z, Rodin AS, Andreev GO, Bao W, McLeod AS, Wagner M, Zhang LM, Zhao Z, Thiemens M, Dominguez G, Fogler MM, Neto AHC, Lau CN, Keilmann F, Basov DN. Gatetuning of graphene plasmons revealed by infrared nanoimaging. Nature 2012, 487, 82–85. Search in Google Scholar
[136] Chen J, Badioli M, AlonsoGonzález P, Thongrattanasiri S, Huth F, Osmond J, Spasenovic M, Centeno A, Pesquera A, Godignon P, Zurutuza A, Camara N, Abajo JGD, Hillenbrand R, Koppens F. Optical nanoimaging of gatetunable graphene plasmons. Nature 2012, 487, 77–81. Search in Google Scholar
[137] Allen Jr S, Tsui D, Logan R. Observation of the twodimensional plasmon in silicon inversion layers. Phys. Rev. Lett. 1977, 38, 980–983. Search in Google Scholar
[138] Batke E, Heitmann D, Tu C. Plasmon and magnetoplasmon excitation in twodimensional electron spacecharge layers on GaAs. Phys. Rev. B 1986, 34, 6951–6960. Search in Google Scholar
[139] Hwang E, Sarma SD. Dielectric function, screening, and plasmons in twodimensional graphene. Phys. Rev. B 2007, 75, 205418. Search in Google Scholar
[140] Ju L, Geng B, Horng J, Girit C, Martin M, Hao Z, Bechtel HA, Liang X, Zettl A, Shen YR, Wang F. Graphene plasmonics for tunable terahertz metamaterials. Nat. Nanotechnol. 2011, 6, 630–634. Search in Google Scholar
[141] Lee SH, Choi M, Kim TT, Lee S, Liu M, Yin X, Choi HK, Lee SS, Choi CG, Choi SY, Zhang X, Min B. Switching terahertz waves with gatecontrolled active graphene metamaterials. Nat. Mater. 2012, 11, 936–941. Search in Google Scholar
[142] Yan H, Li X, Chandra B, Tulevski G, Wu Y, Freitag M, Zhu W, Avouris P, Xia F. Tunable infrared plasmonic devices using graphene/insulator stacks. Nat. Nanotechnol. 2012, 7, 330–334. Search in Google Scholar
[143] Bostwick A, Ohta T, Seyller T, Horn K, Rotenberg E. Quasiparticle dynamics in graphene. Nat. Phys. 2006, 3, 36–40. Search in Google Scholar
[144] Eberlein T, Bangert U, Nair RR, Jones R, Gass M, Bleloch AL, Novoselov KS, Geim A, Briddon PR. Plasmon spectroscopy of freestanding graphene films. Phys. Rev. B 2008, 77, 233406. Search in Google Scholar
[145] Brar VW, Wickenburg S, Panlasigui M, Park CH, Wehling TO, Zhang Y, Decker R, Girit Ç, Balatsky AV, Louie SG, Zettl A, Crommie MF. Observation of carrierdensitydependent manybody effects in graphene via tunneling spectroscopy. Phys. Rev. Lett. 2010, 104, 036805. Search in Google Scholar
[146] Zhou W, Lee J, Nanda J, Pantelides ST, Pennycook SJ, Idrobo JC. Atomically localized plasmon enhancement in monolayer graphene. Nat. Nanotechnol. 2012, 7, 161–165. Search in Google Scholar
[147] Fang Z, Thongrattanasiri S, Schlather A, Liu Z, Ma L, Wang Y, Ajayan PM, Nordlander P, Halas NJ, García de Abajo FJ. Gated tunability and hybridization of localized plasmons in nanostructured graphene. ACS Nano 2013, 7, 2388–2395. Search in Google Scholar
[148] GarciaPomar JL, Nikitin AY, MartinMoreno L. Scattering of graphene plasmons by defects in the graphene sheet. ACS Nano 2013, 7, 4988–4994. Search in Google Scholar
[149] Thongrattanasiri S, de Abajo FJG. Optical field enhancement by strong plasmon interaction in graphene nanostructures. Phys. Rev. Lett. 2013, 110, 187401. Search in Google Scholar
[150] Christensen J, Manjavacas A, Thongrattanasiri S, Koppens FH, Garcì’a de Abajo FJ. Graphene plasmon waveguiding and hybridization in individual and paired nanoribbons. ACS Nano 2011, 6, 431–440. Search in Google Scholar
[151] Yao Y, Kats MA, Genevet P, Yu N, Song Y, Kong J, Capasso F. Broad electrical tuning of grapheneloaded plasmonic antennas. Nano Lett. 2013, 13, 1257–1264. Search in Google Scholar
[152] Papasimakis N, Thongrattanasiri S, Zheludev NI, de Abajo FG. The magnetic response of graphene splitring metamaterials. Light Sci. Appl. 2013, 2, e78. Search in Google Scholar
[153] Yan H, Low T, Zhu W, Wu Y, Freitag M, Li X, Guinea F, Avouris P, Xia F. Damping pathways of midinfrared plasmons in graphene nanostructures. Nat. Photonics 2013, 7, 394–399. Search in Google Scholar
[154] Nair R, Blake P, Grigorenko AN, Novoselov KS, Booth TJ, Stauber T, Peres NMR, Geim AK. Fine structure constant defines visual transparency of graphene. Science 2008, 320, 1308–1308. Search in Google Scholar
[155] Liu N, Mesch M, Weiss T, Hentschel M, Giessen H. Infrared perfect absorber and its application as plasmonic sensor. Nano Lett. 2010, 10, 2342–2348. Search in Google Scholar
[156] Zhu JJ, Badalyan S, Peeters F. Plasmonic excitations in Coulombcoupled Nlayer graphene structures. Phys. Rev. B 2013, 87, 085401. Search in Google Scholar
[157] Li Z, Yu N. Modulation of midinfrared light using graphenemetal plasmonic antennas. Appl. Phys. Lett. 2013, 102, 131108. Search in Google Scholar
[158] Llatser I, Christian K, Albert CA, Miquel JJ, Eduard A, Chigrin DN. Graphenebased nanopatch antenna for terahertz radiation. Phot. Nano. Fund. Appl. 2012, 10, 353–358. Search in Google Scholar
[159] Auditore A, De Angelis C, Locatelli A, Boscolo S, Midrio M, Romagnoli M, Capobianco AD, Nalesso G. Graphene sustained nonlinear modes in dielectric waveguides. Opt. Lett. 2013, 38, 631–633. Search in Google Scholar
[160] Lee SH, Choi J, Kim HD, Choi H, Min B. Ultrafast refractive index control of a terahertz graphene metamaterial. Sci. Rep. 2013, 3, 2135. Search in Google Scholar
[161] Ebbesen TW, Lezec H, Ghaemi H, Thio T, Wolff P. Extraordinary optical transmission through subwavelength hole arrays. Nature 1998, 391, 667–669. Search in Google Scholar
[162] MartinMoreno L, GarcíaVida FJ, Lezec HJ, Pellerin KM, Thio T, Pendry JB, Ebbesen TW. Theory of extraordinary optical transmission through subwavelength hole arrays. Phys. Rev. Lett. 2001, 86, 1114–1117. Search in Google Scholar
[163] Grischkowsky D, Keiding S, van Exter M, Fattinger C. Farinfrared timedomain spectroscopy with terahertz beams of dielectrics and semiconductors. J. Opt. Soc. Am. B 1990, 7, 2006–2015. Search in Google Scholar
[164] Niu J, Jun Shin Y, Lee Y, Ahn JH, Yang H. Graphene induced tunability of the surface plasmon resonance. Appl. Phys. Lett. 2012, 100, 061116. Search in Google Scholar
[165] Kim J, Son H, Cho DJ, Geng B, Regan W, Shi S, Kim K, Zettl A, Shen YR, Wang F. Electrical control of optical plasmon resonance with graphene. Nano Lett. 2012, 12, 5598–5602. Search in Google Scholar
[166] Brar VW, Jang M, Sherrott M, Lopez JJ, Atwater HA. Highly confined tunable midinfrared plasmonics in graphene nanoresonators. Nano Lett. 2013, 13, 2154–2157. Search in Google Scholar
[167] Emani NK, Chung TF, Ni X, Kildishev AV, Chen YP, Boltasseva A. Electrically tunable damping of plasmonic resonances with graphene. Nano Lett. 2012, 12, 5202–5206. Search in Google Scholar
[168] Brolo AG. Plasmonics for future biosensors. Nat. Photonics 2012, 6, 709–713. Search in Google Scholar
[169] West JL, Halas NJ. Engineered nanomaterials for biophotonics applications: improving sensing, imaging, and therapeutics. Annu. Rev. Biomed. Eng. 2003, 5, 285–292. Search in Google Scholar
[170] Homola J. Present and future of surface plasmon resonance biosensors. Anal. Bioanal. Chem. 2003, 377, 528–539. Search in Google Scholar
[171] Homola J. Surface plasmon resonance sensors for detection of chemical and biological species. Chem. Rev. 2008, 108, 462–493. Search in Google Scholar
[172] Willets KA, Van Duyne RP. Localized surface plasmon resonance spectroscopy and sensing. Annu. Rev. Phys. Chem. 2007, 58, 267–297. Search in Google Scholar
[173] Kabashin A, Evans P, Pastkovsky S, Hendren W, Wurtz GA, Atkinson R, Pollard R, Podolskiy VA, Zayats AV. Plasmonic nanorod metamaterials for biosensing. Nat. Mater. 2009, 8, 867–871. Search in Google Scholar
[174] Hendry E, Carpy T, Johnston J, Popland M, Mikhaylovskiy RV, Lapthorn AJ, Kelly SM, Barron LD, Gadegaard N, Kadodwala M. Ultrasensitive detection and characterization of biomolecules using superchiral fields. Nat. Nanotechnol. 2010, 5, 783–787. Search in Google Scholar
[175] Lee J, Hernandez P, Lee J, Govorov AO, Kotov NA. Exciton–plasmon interactions in molecular spring assemblies of nanowires and wavelengthbased protein detection. Nat. Mater. 2007, 6, 291–295. Search in Google Scholar
[176] Wu C, Khanikaev AB, Adato R, Arju N, Yanik AA, Altug H, Shvets G. Fanoresonant asymmetric metamaterials for ultrasensitive spectroscopy and identification of molecular monolayers. Nat. Mater. 2011, 11, 69–75. Search in Google Scholar
[177] Kravets V, Schedin F, Jalil R, Britnell L, Gorbachev RV, Ansell D, Thackray B, Novoselov KS, Geim AK, Kabashin AV, Grigorenko AN. Singular phase nanooptics in plasmonic metamaterials for labelfree singlemolecule detection. Nat. Mater. 2013, 12, 304–309. Search in Google Scholar
[178] Brolo AG, Gordon R, Leathem B, Kavanagh KL. Surface plasmon sensor based on the enhanced light transmission through arrays of nanoholes in gold films. Langmuir 2004, 20, 4813–4815. Search in Google Scholar
[179] Tetz KA, Pang L, Fainman Y. Highresolution surface plasmon resonance sensor based on linewidthoptimized nanohole array transmittance. Opt. Lett. 2006, 31, 1528–1530. Search in Google Scholar
[180] Dahlin AB, Tegenfeldt JO, Höök F. Improving the instrumental resolution of sensors based on localized surface plasmon resonance. Anal. Chem. 2006, 78, 4416–4423. Search in Google Scholar
[181] Abbas A, Linman MJ, Cheng Q. New trends in instrumental design for surface plasmon resonancebased biosensors. Biosens. Bioelectron. 2011, 26, 1815–1824. Search in Google Scholar
[182] Yanik AA, Cetin AE, Huang M, Artar A, Mousavi SH, Khanikaev A, Connor JH, Shvets G, Altug H. Seeing protein monolayers with naked eye through plasmonic Fano resonances. Proc. Natl. Acad. Sci. USA 2011, 108, 11784–11789. Search in Google Scholar
[183] Miroshnichenko AE, Flach S, Kivshar YS. Fano resonances in nanoscale structures. Rev. Mod. Phys. 2010, 82, 2257–2298. Search in Google Scholar
[184] Luk’yanchuk B, Zheludev NI, Maier SA, Halas NJ, Nordlander P, Giessen H, Chong CT. The Fano resonance in plasmonic nanostructures and metamaterials. Nat. Mater. 2010, 9, 707–715. Search in Google Scholar
[185] Shafiei F, Monticone F, Le KQ, Liu XX, Hartsfield T, Alù A, Li X. A subwavelength plasmonic metamolecule exhibiting magneticbased optical Fano resonance. Nat. Nanotechnol. 2013, 8, 95–99. Search in Google Scholar
[186] Fano U. Effects of configuration interaction on intensities and phase shifts. Phys. Rev. 1961, 124, 1866–1878. Search in Google Scholar
[187] Chang WS, Lassiter JB, Swanglap P, Sobhani H, Khatua S, Nordlander P, Halas NJ, Link S. A plasmonic Fano switch. Nano Lett. 2012, 12, 4977–4982. Search in Google Scholar
[188] Argyropoulos C, Chen PY, Monticone F, D’Aguanno G, Alu A. Nonlinear plasmonic cloaks to realize giant alloptical scattering switching. Phys. Rev. Lett. 2012, 108, 263905. Search in Google Scholar
[189] Zheludev NI, Prosvirnin S, Papasimakis N, Fedotov V. Lasing spaser. Nat. Photonics 2008, 2, 351–354. Search in Google Scholar
[190] Luk’yanchuk BS, Chong TC, Shi LP, Tribelsky MI, Wang ZB, Li L, Qiu CW, Sheppard CJR, Wu JH. in PhotonicsGlobal@ Singapore, 2008. IPGC 2008. IEEE. 14 (IEEE). Search in Google Scholar
[191] Hao F, Sonnefraud Y, Van Dorpe P, Maier SA, Halas NJ, Nordlander P. Symmetry breaking in plasmonic nanocavities: subradiant LSPR sensing and a tunable Fano resonance. Nano Lett. 2008, 8, 3983–3988. Search in Google Scholar
[192] Christ A, Martin OJ, Ekinci Y, Gippius NA, Tikhodeev SG. Symmetry breaking in a plasmonic metamaterial at optical wavelength. Nano Lett. 2008, 8, 2171–2175. Search in Google Scholar
[193] Fedotov VA, Rose M, Prosvirnin SL, Papasimakis N, Zheludev NI. Sharp trappedmode resonances in planar metamaterials with a broken structural symmetry. Phys. Rev. Lett. 2007, 99, 147401. Search in Google Scholar
[194] Verellen N, Sonnefraud Y, Sobhani H, Hao F, Moshchalkov VV, Van Dorpe P, Nordlander P, Maier SA. Fano resonances in individual coherent plasmonic nanocavities. Nano Lett. 2009, 9, 1663–1667. Search in Google Scholar
[195] Liu N, Langguth L, Weiss T, Kästel J, Fleischhauer M, Pfau T, Giessen H. Plasmonic analogue of electromagnetically induced transparency at the Drude damping limit. Nat. Mater. 2009, 8, 758–762. Search in Google Scholar
[196] Liu N, Weiss T, Mesch M, Langguth L, Eigenthaler U, Hirscher M, Sönnichsen C, Giessen H. Planar metamaterial analogue of electromagnetically induced transparency for plasmonic sensing. Nano Lett. 2009, 10, 1103–1107. Search in Google Scholar
[197] Ridolfo A, Di Stefano O, Fina N, Saija R, Savasta S. Quantum plasmonics with quantum dotmetal nanoparticle molecules: influence of the Fano effect on photon statistics. Phys. Rev. Lett. 2010, 105, 263601. Search in Google Scholar
[198] Becker J, Trügler A, Jakab A, Hohenester U, Sönnichsen C. The optimal aspect ratio of gold nanorods for plasmonic biosensing. Plasmonics 2010, 5, 161–167. Search in Google Scholar
[199] Mayer KM, Lee S, Liao H, Rostro BC, Fuentes A, Scully PT, Nehl CL, Hafner JH. A labelfree immunoassay based upon localized surface plasmon resonance of gold nanorods. ACS Nano 2008, 2, 687–692. Search in Google Scholar
[200] Simovski CR, Belov PA, Atrashchenko AV, Kivshar YS. Wire metamaterials: physics and applications. Adv. Mater. 2012, 24, 4229–4248. Search in Google Scholar
[201] KuwataGonokami M, Saito N, Ino Y, Kauranen M, Jefimovs K, Vallius T, Turunen J, Svirko Y. Giant optical activity in quasitwodimensional planar nanostructures. Phys. Rev. Lett. 2005, 95, 227401. Search in Google Scholar
[202] Schäferling M, Dregely D, Hentschel M, Giessen H. Tailoring enhanced optical chirality: design principles for chiral plasmonic nanostructures. Phys. Rev. X 2012, 2, 031010. Search in Google Scholar
[203] Tang Y, Cohen AE. Optical chirality and its interaction with matter. Phys. Rev. Lett. 2010, 104, 163901. Search in Google Scholar
[204] Barron LD. Molecular Light Scattering and Optical Activity, 2nd ed., Cambridge University Press: Cambridge, 2004. Search in Google Scholar
[205] Tan SJ, Campolongo MJ, Luo D, Cheng W. Building plasmonic nanostructures with DNA. Nat. Nanotechnol. 2011, 6, 268–276. Search in Google Scholar
[206] Bishop KJ, Wilmer CE, Soh S, Grzybowski BA. Nanoscale forces and their uses in selfassembly. Small 2009, 5, 1600–1630. Search in Google Scholar
[207] Gong J, Li G, Tang Z. Selfassembly of noble metal nanocrystals: fabrication, optical property, and application. Nano Today 2012, 7, 564–585. Search in Google Scholar
[208] Fan JA, Wu C, Bao K, Bao J, Bardhan R, Halas NJ, Manoharan VN, Nordlander P, Shvets G, Capasso F. Selfassembled plasmonic nanoparticle clusters. Science 2010, 328, 1135–1138. Search in Google Scholar
[209] Prodan E, Radloff C, Halas N, Nordlander P. A hybridization model for the plasmon response of complex nanostructures. Science 2003, 302, 419–422. Search in Google Scholar
[210] Nordlander P, Oubre C, Prodan E, Li K, Stockman M. Plasmon hybridization in nanoparticle dimers. Nano Lett. 2004, 4, 899–903. Search in Google Scholar
[211] Kuzyk A, Schreiber R, Fan Z, Pardatscher G, Roller EM, Högele A, Simmel FC, Govorov AO, Liedl T. DNAbased selfassembly of chiral plasmonic nanostructures with tailored optical response. Nature 2012, 483, 311–314. Search in Google Scholar
[212] Rothemund PW. Folding DNA to create nanoscale shapes and patterns. Nature 2006, 440, 297–302. Search in Google Scholar
[213] Mirkin CA, Letsinger RL, Mucic RC, Storhoff JJ. A DNAbased method for rationally assembling nanoparticles into macroscopic materials. Nature 1996, 382, 607–609. Search in Google Scholar
[214] Alivisatos AP, Johnsson KP, Peng X, Wilson TE, Loweth CJ, Bruchez MP Jr, Schultz PG. Organization of ‘nanocrystal molecules’ using DNA. Nature 1996, 382, 609–611. Search in Google Scholar
[215] Mastroianni A, Claridge S, Alivisatos AP. Pyramidal and chiral groupings of gold nanocrystals assembled using DNA scaffolds. J. Am. Chem. Soc. 2009, 131, 8455–8459. Search in Google Scholar
[216] Mucic RC, Storhoff JJ, Mirkin CA, Letsinger RL. DNAdirected synthesis of binary nanoparticle network materials. J. Am. Chem. Soc. 1998, 120, 12674–12675. Search in Google Scholar
[217] Aldaye FA, Sleiman HF. Sequential selfassembly of a DNA hexagon as a template for the organization of gold nanoparticles. Angew. Chem. Int. Ed. 2006, 45, 2204–2209. Search in Google Scholar
[218] Murray C, Kagan C, Bawendi M. Synthesis and characterization of monodisperse nanocrystals and closepacked nanocrystal assemblies. Annu. Rev. Mater. Sci. 2000, 30, 545–610. Search in Google Scholar
[219] Whitesides GM, Grzybowski B. Selfassembly at all scales. Science 2002, 295, 2418–2421. Search in Google Scholar
[220] Tao A, Sinsermsuksakul P, Yang P. Tunable plasmonic lattices of silver nanocrystals. Nat. Nanotechnol. 2007, 2, 435–440. Search in Google Scholar
[221] Chen CF, Tzeng SD, Chen HY, Lin KJ, Gwo S. Tunable plasmonic response from alkanethiolatestabilized gold nanoparticle superlattices: evidence of nearfield coupling. J. Am. Chem. Soc. 2008, 130, 824–826. Search in Google Scholar
[222] Lin MH, Chen HY, Gwo S. Layerbylayer assembly of threedimensional colloidal supercrystals with tunable plasmonic properties. J. Am. Chem. Soc. 2010, 132, 11259–11263. Search in Google Scholar
[223] Dong A, Ye X, Chen J, Murray CB. Twodimensional binary and ternary nanocrystal superlattices: the case of monolayers and bilayers. Nano Lett. 2011, 11, 1804–1809. Search in Google Scholar
[224] Henzie J, Grünwald M, WidmerCooper A, Geissler PL, Yang P. Selfassembly of uniform polyhedral silver nanocrystals into densest packings and exotic superlattices. Nat. Mater. 2011, 11, 131–137. Search in Google Scholar
[225] Leunissen ME, Christova CG, Hynninen AP, Royall CP, Campbell AI, Imhof A, Dijkstra M, van Roij R, van Blaaderen A. Ionic colloidal crystals of oppositely charged particles. Nature 2005, 437, 235–240. Search in Google Scholar
[226] Shevchenko EV, Talapin DV, Kotov NA, O’Brien S, Murray CB. Structural diversity in binary nanoparticle superlattices. Nature 2006, 439, 55–59. Search in Google Scholar
[227] Dong A, Chen J, Vora PM, Kikkawa JM, Murray CB. Binary nanocrystal superlattice membranes selfassembled at the liquidair interface. Nature 2010, 466, 474–477. Search in Google Scholar
[228] Tao AR, Habas S, Yang P. Shape control of colloidal metal nanocrystals. Small 2008, 4, 310–325. Search in Google Scholar
[229] Nahata A, Linke RA, Ishi T, Ohashi K. Enhanced nonlinear optical conversion from a periodically nanostructured metal film. Opt. Lett. 2003, 28, 423–425. Search in Google Scholar
[230] Kim S, Jin J, Kim YJ, Park IY, Kim Y, Kim SW. Highharmonic generation by resonant plasmon field enhancement. Nature 2008, 453, 757–760. Search in Google Scholar
[231] Park IY, Kim S, Choi J, Lee DH, Kim YJ, Kling MF, Stockman MI, Kim SW. Plasmonic generation of ultrashort extremeultraviolet light pulses. Nat. Photonics 2011, 5, 677–681. Search in Google Scholar
[232] Klein MW, Enkrich C, Wegener M, Linden, S. Secondharmonic generation from magnetic metamaterials. Science 2006, 313, 502–504. Search in Google Scholar
[233] Klein MW, Wegener M, Feth N, Linden S. Experiments on second and thirdharmonic generation from magnetic metamaterials. Opt. Exp. 2007, 15, 5238–5247. Search in Google Scholar
[234] Maslovski S, Tretyakov S. Phase conjugation and perfect lensing. J. Appl. Phys. 2003, 94, 4241–4243. Search in Google Scholar
[235] Pendry J. Time reversal and negative refraction. Science 2008, 322, 71–73. Search in Google Scholar
[236] Katko AR, Gu S, Barrett JP, Popa BI, Shvets G, Cummer SA. Phase conjugation and negative refraction using nonlinear active metamaterials. Phys. Rev. Lett. 2010, 105, 123905. Search in Google Scholar
[237] Palomba S, Zhang S, Park Y, Bartal G, Yin X, Zhang X. Optical negative refraction by fourwave mixing in thin metallic nanostructures. Nat. Mater. 2011, 11, 34–38. Search in Google Scholar
[238] Harutyunyan H, Beams R, Novotny L. Controllable optical negative refraction and phase conjugation in graphite thin films. Nat. Phys. 2013, 9, 423–425. Search in Google Scholar
[239] Zharov AA, Shadrivov IV, Kivshar YS. Nonlinear properties of lefthanded metamaterials. Phys. Rev. Lett. 2003, 91, 037401. Search in Google Scholar
[240] Agranovich V, Shen Y, Baughman R, Zakhidov A. Linear and nonlinear wave propagation in negative refraction metamaterials. Phys. Rev. B 2004, 69, 165112. Search in Google Scholar
[241] Lazarides N, Eleftheriou M, Tsironis G. Discrete breathers in nonlinear magnetic metamaterials. Phys. Rev. Lett. 2006, 97, 157406. Search in Google Scholar
[242] Liu Y, Bartal G, Genov DA, Zhang X. Subwavelength discrete solitons in nonlinear metamaterials. Phys. Rev. Lett. 2007, 99, 153901. Search in Google Scholar
[243] Wurtz GA, Pollard R, Hendren W, Wiederrecht GP, Gosztola DJ, Podolskiy VA, Zayats AV. Designed ultrafast optical nonlinearity in a plasmonic nanorod metamaterial enhanced by nonlocality. Nat. Nanotechnol. 2011, 6, 107–111. Search in Google Scholar
[244] Krasavin AV, Vo TP, Dickson W, Bolger PM, Zayats AV. Allplasmonic modulation via stimulated emission of copropagating surface plasmon polaritons on a substrate with gain. Nano Lett. 2011, 11, 2231–2235. Search in Google Scholar
[245] Ren M, Plum E, Xu J, Zheludev NI. Giant nonlinear optical activity in a plasmonic metamaterial. Nat. Commun. 2012, 3, 833. Search in Google Scholar
[246] Lapine M, Shadrivov IV, Powell DA, Kivshar YS. Magnetoelastic metamaterials. Nat. Mater. 2011, 11, 30–33. Search in Google Scholar
[247] Tame MS, McEnery KR, Özdemir SK, Lee J, Maier SA, Kim MS. Quantum plasmonics. Nat. Phys. 2013, 9, 329–340. Search in Google Scholar
[248] Altewischer E, Van Exter M, Woerdman J. Plasmonassisted transmission of entangled photons. Nature 2002, 418, 304–306. Search in Google Scholar
[249] Ouyang F, Batson P, Isaacson M. Quantum size effects in the surfaceplasmon excitation of small metallic particles by electronenergyloss spectroscopy. Phys. Rev. B 1992, 46, 15421. Search in Google Scholar
[250] Scholl JA, Koh AL, Dionne JA. Quantum plasmon resonances of individual metallic nanoparticles. Nature 2012, 483, 421–427. Search in Google Scholar
[251] Savage KJ, Hawkeye MM, Esteban R, Borisov AG, Aizpurua J, Baumberg JJ. Revealing the quantum regime in tunnelling plasmonics. Nature 2012, 491, 574–577. Search in Google Scholar
[252] Scholl JA, GarcíaEtxarri A, Koh AL, Dionne JA. Observation of quantum tunneling between two plasmonic nanoparticles. Nano Lett. 2013, 13, 564–569. Search in Google Scholar
[253] García de Abajo FJ. Nonlocal effects in the plasmons of strongly interacting nanoparticles, dimers, and waveguides. J. Phys. Chem. C 2008, 112, 17983–17987. Search in Google Scholar
[254] FernándezDomínguez A, Wiener A, GarcíaVidal F, Maier S, Pendry J. Transformationoptics description of nonlocal effects in plasmonic nanostructures. Phys. Rev. Lett. 2012, 108, 106802. Search in Google Scholar
[255] Esteban R, Borisov AG, Nordlander P, Aizpurua J. Bridging quantum and classical plasmonics with a quantumcorrected model. Nat. Commun. 2012, 3, 825. Search in Google Scholar
[256] Jacob Z, Kim JY, Naik GV, Boltasseva A, Narimanov EE, Shalaev VM. Engineering photonic density of states using metamaterials. Appl. Phys. B 2010, 100, 215–218. Search in Google Scholar
[257] Noginov MA, Zhu G, Belgrave AM, Bakker R, Shalaev VM, Narimanov EE, Stout S, Herz E, Suteewong T, Wiesner U. Demonstration of a spaserbased nanolaser. Nature 2009, 460, 1110–1112. Search in Google Scholar
[258] Oulton RF, Sorger VJ, Zentgraf T, Ma RM, Gladden C, Dai L, Bartal G, Zhang X. Plasmon lasers at deep subwavelength scale. Nature 2009, 461, 629–632. Search in Google Scholar
[259] Akimov AV, Mukherjee A, Yu CL, Chang DE, Zibrov AS, Hemmer PR, Park H, Lukin MD. Generation of single optical plasmons in metallic nanowires coupled to quantum dots. Nature 2007, 450, 402–406. Search in Google Scholar
[260] Chang DE, Sørensen AS, Demler EA, Lukin MD. A singlephoton transistor using nanoscale surface plasmons. Nat. Phys. 2007, 3, 807–812. Search in Google Scholar
[261] Falk AL, Koppens FHL, Yu CL, Kang K, de Leon Snapp N, Akimov AV, Jo MH, Lukin MD, Park H. Nearfield electrical detection of optical plasmons and singleplasmon sources. Nat. Phys. 2009, 5, 475–479. Search in Google Scholar
[262] Driscoll T, Kim HT, Chae BG, Kim BJ, Lee YW, Jokerst NM, Palit S, Smith DR, Di Ventra M, Basov DN. Memory metamaterials. Science 2009, 325, 1518–1521. Search in Google Scholar
[263] Liu M, Hwang HY, Tao H, Strikwerda AC, Fan K, Keiser GR, Sternbach AJ, West KG, Kittiwatanakul S, Lu J, Wolf SA, Omenetto FG, Zhang X, Nelson KA, Averitt RD. Terahertzfieldinduced insulatortometal transition in vanadium dioxide metamaterial. Nature 2012, 487, 345–348. Search in Google Scholar
[264] Wang J, Liu S, Nahata A. Reconfigurable plasmonic devices using liquid metals. Opt. Exp. 2012, 20, 12119–12126. Search in Google Scholar
[265] Khoo I, Werner D, Liang X, Diaz A, Weiner B. Nanosphere dispersed liquid crystals for tunable negativezeropositive index of refraction in the optical and terahertz regimes. Opt. Lett. 2006, 31, 2592–2594. Search in Google Scholar
[266] Liu Q, Cui Y, Gardner D, Li X, He S, Smalyukh II. Selfalignment of plasmonic gold nanorods in reconfigurable anisotropic fluids for tunable bulk metamaterial applications. Nano Lett. 2010, 10, 1347–1353. Search in Google Scholar
[267] Urzhumov Y, Lee JS, Tyler T, Dhar S, Nguyen V, Jokerst NM, Schmalenberg P, Smith DR. Electronically reconfigurable metalonsilicon metamaterial. Phys. Rev. B 2012, 86, 075112. Search in Google Scholar
[268] Liu A, Zhu W, Tsai D, Zheludev, N. Micromachined tunable metamaterials: a review. J. Opt. 2012, 14, 114009. Search in Google Scholar
[269] Ou JY, Plum E, Zhang J, Zheludev NI. An electromechanically reconfigurable plasmonic metamaterial operating in the nearinfrared. Nat. Nanotechnol. 2013, 8, 252–255. Search in Google Scholar
[270] Zhao C, Liu Y, Zhao Y, Fang N, Huang TJ. A reconfigurable plasmofluidic lens. Nat. Commun. 2013, 4, 2305. Search in Google Scholar
©2014 by Walter de Gruyter Berlin/Boston
This article is distributed under the terms of the Creative Commons Attribution NonCommercial License, which permits unrestricted noncommercial use, distribution, and reproduction in any medium, provided the original work is properly cited.